#------------------------------------------------------------------------------
#$Date: 2016-03-23 22:21:53 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179478 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/75/4337513.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4337513
loop_
_publ_author_name
'Holland, Michael'
'Donakowski, Martin D.'
'Pozzi, Eric A.'
'Rasmussen, Andrew M.'
'Tran, Thanh Thao'
'Pease-Dodson, Shannon E'
'Halasyamani, P. Shiv'
'Seideman, Tamar'
'Van Duyne, Richard P.'
'Poeppelmeier, Kenneth R.'
_publ_section_title
;
 Polar alignment of Λ-shaped basic building units within transition metal
 oxide fluoride materials.
;
_journal_issue                   1
_journal_name_full               'Inorganic chemistry'
_journal_page_first              221
_journal_page_last               228
_journal_paper_doi               10.1021/ic402177j
_journal_volume                  53
_journal_year                    2014
_chemical_absolute_configuration ad
_chemical_formula_moiety         'F14 Mo4 O8, F7 Mo2 O4, 2.0(I), 10(K)'
_chemical_formula_sum            'F21 I2 K10 Mo6 O12'
_chemical_formula_weight         1811.31
_chemical_name_systematic
;
 ? 
;
_space_group_crystal_system      orthorhombic
_space_group_IT_number           31
_space_group_name_Hall           'P 2ac -2'
_symmetry_space_group_name_Hall  'P 2ac -2'
_symmetry_space_group_name_H-M   'P m n 21'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_date             2013-06-11
_audit_creation_method
;
  Olex2 1.1
  (compiled Nov  1 2011 20:42:30, GUI svn.r3906)
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   20.0720(8)
_cell_length_b                   7.7549(3)
_cell_length_c                   11.4644(4)
_cell_measurement_temperature    99.97
_cell_volume                     1784.51(12)
_computing_cell_refinement       'SAINT V7.23A (Bruker, 2005)'
_computing_data_collection       'APEX2 V2.1-4 (Bruker, 2007)'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics
;
O. V. Dolomanov, L. J. Bourhis, R. J. Gildea, J. A. K. Howard and H. Puschmann,
OLEX2: a complete structure solution, refinement and analysis program.
J. Appl. Cryst. (2009). 42, 339-341.
;
_computing_publication_material
;
O. V. Dolomanov, L. J. Bourhis, R. J. Gildea, J. A. K. Howard and H. Puschmann,
OLEX2: a complete structure solution, refinement and analysis program.
J. Appl. Cryst. (2009). 42, 339-341.
;
_computing_structure_refinement
;
XL, G.M. Sheldrick, Acta Cryst.
(2008). A64, 112-122
;
_computing_structure_solution
;
XS, G.M. Sheldrick, Acta Cryst.
(2008). A64, 112-122
;
_diffrn_ambient_temperature      99.97
_diffrn_detector_area_resol_mean 8
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker Kappa APEX CCD area detector'
_diffrn_measurement_method       'ω and φ scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0672
_diffrn_reflns_av_unetI/netI     0.0275
_diffrn_reflns_limit_h_max       28
_diffrn_reflns_limit_h_min       -28
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -10
_diffrn_reflns_limit_l_max       16
_diffrn_reflns_limit_l_min       -16
_diffrn_reflns_number            72517
_diffrn_reflns_theta_full        30.03
_diffrn_reflns_theta_max         30.03
_diffrn_reflns_theta_min         2.03
_diffrn_source                   'sealed tube'
_diffrn_source_current           30.0
_diffrn_source_power             1.5
_diffrn_source_voltage           50.0
_exptl_absorpt_coefficient_mu    5.092
_exptl_absorpt_correction_T_max  0.8833
_exptl_absorpt_correction_T_min  0.3467
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Bruker)'
_exptl_crystal_colour            'clear brown'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_primary    brown
_exptl_crystal_density_diffrn    3.371
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             1665.9
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.07
_exptl_crystal_size_min          0.03
_refine_diff_density_max         5.545
_refine_diff_density_min         -2.117
_refine_diff_density_rms         0.259
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.00(8)
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.067
_refine_ls_matrix_type           full
_refine_ls_number_parameters     255
_refine_ls_number_reflns         5358
_refine_ls_number_restraints     2
_refine_ls_restrained_S_all      1.067
_refine_ls_R_factor_all          0.0470
_refine_ls_R_factor_gt           0.0427
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0782P)²+5.5784P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1152
_refine_ls_wR_factor_ref         0.1186
_reflns_number_gt                4916
_reflns_number_total             5358
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic402177j_si_008.cif
_cod_data_source_block           Compound_8
_cod_database_code               4337513
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 'x, y, z'
2 '-x+1/2, -y, z+1/2'
3 '-x, y, z'
4 'x+1/2, -y, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
I2D I 0.5000 0.75348(17) 0.83773(8) 0.0270(2) Uani 0.6451(19) 2 d SP
I6D I 0.5000 1.3661(4) 0.82559(16) 0.0270(2) Uani 0.331(2) 2 d SP
I1D I 0.5000 0.5232(5) 0.8305(2) 0.0270(2) Uani 0.229(2) 2 d SP
I3D I 0.5000 0.9873(5) 0.8263(3) 0.0270(2) Uani 0.228(2) 2 d SP
I4D I 0.5000 1.1348(4) 0.82915(16) 0.0270(2) Uani 0.329(2) 2 d SP
I5D I 0.5000 1.2517(6) 0.8262(2) 0.0270(2) Uani 0.237(2) 2 d SP
Mo1 Mo 0.30285(3) 0.04444(8) 0.02989(5) 0.01721(13) Uani 1 1 d .
Mo2 Mo 0.19857(3) 0.50244(8) 0.14092(5) 0.01460(12) Uani 1 1 d .
Mo3 Mo 0.5000 0.03279(11) 0.44594(7) 0.01498(16) Uani 1 2 d S
Mo4 Mo 0.5000 0.57158(11) 0.23065(7) 0.01823(17) Uani 1 2 d S
K1 K 0.32785(7) 0.26373(17) 0.32020(13) 0.0173(3) Uani 1 1 d .
K2 K 0.15799(8) 0.23366(18) -0.14494(13) 0.0195(3) Uani 1 1 d .
K3 K 0.15063(9) 0.0395(2) 0.20967(14) 0.0229(3) Uani 1 1 d .
K4 K 0.13778(10) 0.4911(2) 0.48955(15) 0.0252(3) Uani 1 1 d .
K5 K 0.5000 0.0331(3) 0.1191(2) 0.0238(4) Uani 1 2 d S
K6 K 0.0000 0.4274(3) 0.0478(2) 0.0234(4) Uani 1 2 d S
F1 F 0.4337(2) 0.7108(6) 0.1598(4) 0.0219(9) Uani 0.75 1 d P
F2 F 0.5665(2) 0.0672(6) 0.3221(4) 0.0257(10) Uani 0.75 1 d P
F3 F 0.4320(2) 0.4925(5) 0.3371(4) 0.0159(8) Uani 0.75 1 d P
F4 F 0.3758(2) 0.1791(6) 0.0906(4) 0.0185(8) Uani 0.75 1 d P
F5 F 0.3025(2) 0.1796(6) -0.1039(4) 0.0225(9) Uani 0.75 1 d P
F6 F 0.2882(2) 0.5536(6) 0.1920(4) 0.0204(9) Uani 0.75 1 d P
F7 F 0.2861(2) 0.0291(6) 0.4915(4) 0.0186(8) Uani 0.75 1 d P
F8 F 0.2722(2) 0.4551(6) 0.4817(4) 0.0227(9) Uani 0.75 1 d P
F9 F 0.2483(2) 0.2596(5) 0.1018(4) 0.0196(8) Uani 1 1 d .
F10 F 0.2127(2) 0.0259(5) -0.3084(4) 0.0168(8) Uani 0.75 1 d P
F11 F 0.1847(2) 0.3807(6) 0.2828(4) 0.0221(9) Uani 0.75 1 d P
F12 F 0.1268(2) 0.3757(7) 0.0725(4) 0.0257(10) Uani 0.75 1 d P
F13 F 0.4333(3) -0.0701(7) 0.5304(5) 0.0333(11) Uani 0.75 1 d P
F14 F 0.5000 0.7800(8) 0.3582(6) 0.0251(13) Uani 1 2 d S
O1 O 0.4337(2) 0.7108(6) 0.1598(4) 0.0219(9) Uani 0.25 1 d P
O2 O 0.5665(2) 0.0672(6) 0.3221(4) 0.0257(10) Uani 0.25 1 d P
O3 O 0.4320(2) 0.4925(5) 0.3371(4) 0.0159(8) Uani 0.25 1 d P
O4 O 0.3758(2) 0.1791(6) 0.0906(4) 0.0185(8) Uani 0.25 1 d P
O5 O 0.3025(2) 0.1796(6) -0.1039(4) 0.0225(9) Uani 0.25 1 d P
O6 O 0.2882(2) 0.5536(6) 0.1920(4) 0.0204(9) Uani 0.25 1 d P
O7 O 0.2861(2) 0.0291(6) 0.4915(4) 0.0186(8) Uani 0.25 1 d P
O8 O 0.2722(2) 0.4551(6) 0.4817(4) 0.0227(9) Uani 0.25 1 d P
O10 O 0.2127(2) 0.0259(5) -0.3084(4) 0.0168(8) Uani 0.25 1 d P
O11 O 0.1847(2) 0.3807(6) 0.2828(4) 0.0221(9) Uani 0.25 1 d P
O12 O 0.1268(2) 0.3757(7) 0.0725(4) 0.0257(10) Uani 0.25 1 d P
O13 O 0.4333(3) -0.0701(7) 0.5304(5) 0.0333(11) Uani 0.25 1 d P
O16 O 0.1611(3) 0.6897(8) 0.1674(5) 0.0256(11) Uani 1 1 d .
O17 O 0.3439(3) -0.1275(7) -0.0195(5) 0.0255(11) Uani 1 1 d .
O18 O 0.5000 0.2324(10) 0.5031(7) 0.033(2) Uani 1 2 d S
O19 O 0.5000 0.4054(10) 0.1386(7) 0.0249(14) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
I I -0.4742 1.8119 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
I6D I2D K3 114.35(4) 1_545 4_565
I6D I2D K3 114.35(4) 1_545 2_565
I6D I2D K4 61.31(4) 1_545 2_565
I6D I2D K4 61.31(4) 1_545 4_565
I6D I2D K5 126.57(6) 1_545 1_566
I6D I2D K6 64.47(6) 1_545 2_565
I1D I2D I3D 173.18(16) . .
I1D I2D I4D 175.42(11) . .
I1D I2D K3 114.34(6) . 2_565
I1D I2D K3 114.34(6) . 4_565
I1D I2D K4 61.32(6) . 4_565
I1D I2D K4 61.32(6) . 2_565
I1D I2D K5 126.59(11) . 1_566
I1D I2D K6 64.44(11) . 2_565
I3D I2D I6D 173.20(11) . 1_545
I3D I2D K3 62.71(5) . 4_565
I3D I2D K3 62.71(5) . 2_565
I3D I2D K4 122.27(6) . 4_565
I3D I2D K4 122.27(6) . 2_565
I3D I2D K5 60.23(11) . 1_566
I3D I2D K6 108.74(11) . 2_565
I4D I2D I6D 175.44(6) . 1_545
I4D I2D K3 63.65(4) . 2_565
I4D I2D K3 63.65(4) . 4_565
I4D I2D K4 121.13(4) . 4_565
I4D I2D K4 121.13(4) . 2_565
I4D I2D K5 57.99(5) . 1_566
I4D I2D K6 110.98(6) . 2_565
K3 I2D K3 108.52(6) 4_565 2_565
K3 I2D K4 78.69(4) 4_565 4_565
K3 I2D K4 172.79(4) 2_565 4_565
K3 I2D K4 172.79(4) 4_565 2_565
K3 I2D K4 78.69(4) 2_565 2_565
K3 I2D K5 94.97(4) 4_565 1_566
K3 I2D K5 94.97(4) 2_565 1_566
K4 I2D K4 94.10(6) 2_565 4_565
K4 I2D K5 84.13(4) 2_565 1_566
K4 I2D K5 84.13(4) 4_565 1_566
K6 I2D K3 78.72(4) 2_565 2_565
K6 I2D K3 78.72(4) 2_565 4_565
K6 I2D K4 103.25(4) 2_565 2_565
K6 I2D K4 103.25(4) 2_565 4_565
K6 I2D K5 168.97(6) 2_565 1_566
I2D I6D K4 70.20(6) 1_565 4_575
I2D I6D K4 70.20(6) 1_565 2_575
I2D I6D K6 65.97(6) 1_565 2_575
I1D I6D I3D 177.23(19) 1_565 .
I1D I6D I4D 176.1(2) 1_565 .
I1D I6D K4 70.22(10) 1_565 4_575
I1D I6D K4 70.22(10) 1_565 2_575
I1D I6D K6 65.94(16) 1_565 2_575
I3D I6D I2D 177.19(9) . 1_565
I3D I6D K4 108.23(7) . 4_575
I3D I6D K4 108.23(7) . 2_575
I3D I6D K6 116.84(10) . 2_575
I4D I6D I2D 176.04(11) . 1_565
I4D I6D K4 107.58(7) . 2_575
I4D I6D K4 107.58(7) . 4_575
I4D I6D K6 117.99(11) . 2_575
I5D I6D I2D 176.9(3) . 1_565
I5D I6D I1D 176.9(3) . 1_565
I5D I6D K4 108.08(15) . 2_575
I5D I6D K4 108.08(15) . 4_575
I5D I6D K6 117.1(2) . 2_575
K4 I6D K4 103.46(8) 4_575 2_575
K4 I6D K6 109.61(6) 2_575 2_575
K4 I6D K6 109.61(6) 4_575 2_575
I2D I1D I4D 177.61(16) . 1_545
I2D I1D I5D 178.66(19) . 1_545
I2D I1D K4 90.44(9) . 2_565
I2D I1D K4 90.44(9) . 4_565
I2D I1D K6 85.93(12) . 2_565
I6D I1D I2D 179.9(2) 1_545 .
I6D I1D K4 89.53(11) 1_545 2_565
I6D I1D K4 89.53(11) 1_545 4_565
I6D I1D K6 94.13(18) 1_545 2_565
I4D I1D K4 88.25(8) 1_545 4_565
I4D I1D K4 88.25(8) 1_545 2_565
I4D I1D K6 96.46(11) 1_545 2_565
I5D I1D K4 88.83(9) 1_545 2_565
I5D I1D K4 88.83(9) 1_545 4_565
I5D I1D K6 95.41(14) 1_545 2_565
K4 I1D K4 113.09(10) 4_565 2_565
K6 I1D K4 123.39(5) 2_565 4_565
K6 I1D K4 123.39(5) 2_565 2_565
I2D I3D I6D 176.01(16) . .
I2D I3D I5D 175.9(2) . .
I2D I3D K3 88.10(9) . 4_565
I2D I3D K3 88.10(9) . 2_565
I2D I3D K5 91.90(12) . 1_566
I6D I3D K3 93.53(8) . 4_565
I6D I3D K3 93.53(8) . 2_565
I6D I3D K5 84.11(10) . 1_566
I4D I3D I2D 174.2(3) . .
I4D I3D K3 94.25(10) . 4_565
I4D I3D K5 82.30(19) . 1_566
I5D I3D K3 93.57(9) . 2_565
I5D I3D K3 93.57(9) . 4_565
I5D I3D K5 83.99(14) . 1_566
K3 I3D K3 131.79(10) 2_565 4_565
K3 I3D K5 114.07(5) 4_565 1_566
K3 I3D K5 114.07(5) 2_565 1_566
I2D I4D I1D 177.81(9) . 1_565
I2D I4D K3 68.64(6) . 2_565
I2D I4D K3 68.64(6) . 4_565
I2D I4D K5 74.75(7) . 1_566
I6D I4D I2D 179.40(11) . .
I6D I4D K3 111.61(7) . 4_565
I6D I4D K3 111.61(7) . 2_565
I6D I4D K5 104.65(11) . 1_566
I1D I4D K3 112.27(6) 1_565 4_565
I1D I4D K3 112.27(6) 1_565 2_565
I1D I4D K5 103.07(9) 1_565 1_566
I3D I4D I6D 177.0(2) . .
I3D I4D I1D 178.6(2) . 1_565
I3D I4D K3 67.17(9) . 2_565
I3D I4D K3 67.17(9) . 4_565
I3D I4D K5 78.30(18) . 1_566
I5D I4D I2D 179.7(3) . .
I5D I4D I3D 176.2(3) . .
I5D I4D K3 111.25(11) . 4_565
I5D I4D K3 111.25(11) . 2_565
I5D I4D K5 105.5(2) . 1_566
K3 I4D K3 115.05(9) 2_565 4_565
K5 I4D K3 106.55(6) 1_566 4_565
K5 I4D K3 106.55(6) 1_566 2_565
I6D I5D I3D 179.6(3) . .
I6D I5D I4D 178.3(4) . .
I6D I5D K3 124.16(12) . 2_565
I6D I5D K3 124.16(12) . 4_565
I6D I5D K4 59.40(14) . 4_575
I6D I5D K4 59.40(14) . 2_575
I6D I5D K5 117.2(3) . 1_566
I6D I5D K6 51.6(2) . 2_575
I1D I5D K3 124.87(8) 1_565 2_565
I1D I5D K3 124.87(8) 1_565 4_565
I1D I5D K4 58.41(8) 1_565 4_575
I1D I5D K4 58.41(8) 1_565 2_575
I1D I5D K5 115.45(14) 1_565 1_566
I1D I5D K6 53.39(11) 1_565 2_575
I3D I5D I1D 178.6(2) . 1_565
I3D I5D K3 55.68(7) . 2_565
I3D I5D K3 55.68(7) . 4_565
I3D I5D K4 120.83(10) . 2_575
I3D I5D K4 120.83(10) . 4_575
I3D I5D K5 63.18(13) . 1_566
I3D I5D K6 127.98(15) . 2_575
I4D I5D I1D 176.5(3) . 1_565
I4D I5D K3 56.56(11) . 4_565
I4D I5D K3 56.56(11) . 2_565
I4D I5D K4 119.62(15) . 2_575
I4D I5D K4 119.62(15) . 4_575
I4D I5D K5 61.1(2) . 1_566
I4D I5D K6 130.1(3) . 2_575
K3 I5D K3 98.11(10) 2_565 4_565
K3 I5D K6 94.80(6) 4_565 2_575
K3 I5D K6 94.80(6) 2_565 2_575
K4 I5D K3 170.67(9) 2_575 4_565
K4 I5D K3 85.01(4) 2_575 2_565
K4 I5D K3 170.67(9) 4_575 2_565
K4 I5D K3 85.01(4) 4_575 4_565
K4 I5D K4 90.61(10) 4_575 2_575
K4 I5D K6 93.69(9) 2_575 2_575
K4 I5D K6 93.69(9) 4_575 2_575
K5 I5D K3 92.50(8) 1_566 4_565
K5 I5D K3 92.50(8) 1_566 2_565
K5 I5D K4 78.54(6) 1_566 4_575
K5 I5D K4 78.54(6) 1_566 2_575
K5 I5D K6 168.84(13) 1_566 2_575
K3 Mo1 K1 67.76(4) . .
F4 Mo1 K1 48.42(13) . .
F4 Mo1 K3 115.68(13) . .
F4 Mo1 F9 80.13(17) . .
F4 Mo1 F10 86.00(18) . 2
F4 Mo1 O10 86.00(18) . 2
F5 Mo1 K1 118.35(15) . .
F5 Mo1 K3 117.68(14) . .
F5 Mo1 F4 89.72(19) . .
F5 Mo1 F7 88.55(19) . 2_554
F5 Mo1 F9 82.97(18) . .
F5 Mo1 F10 159.8(2) . 2
F5 Mo1 O7 88.55(19) . 2_554
F5 Mo1 O10 159.8(2) . 2
F7 Mo1 K1 117.31(14) 2_554 .
F7 Mo1 K3 49.92(13) 2_554 .
F7 Mo1 F4 161.26(19) 2_554 .
F7 Mo1 F9 81.14(18) 2_554 .
F7 Mo1 F10 89.22(19) 2_554 2
F7 Mo1 O10 89.22(19) 2_554 2
F9 Mo1 K1 51.82(11) . .
F9 Mo1 K3 51.26(12) . .
F10 Mo1 K1 46.44(13) 2 .
F10 Mo1 K3 48.35(13) 2 .
F10 Mo1 F9 76.86(17) 2 .
O7 Mo1 K1 117.31(14) 2_554 .
O7 Mo1 K3 49.92(13) 2_554 .
O7 Mo1 F4 161.26(19) 2_554 .
O7 Mo1 F7 0.0(3) 2_554 2_554
O7 Mo1 F9 81.14(18) 2_554 .
O7 Mo1 F10 89.22(19) 2_554 2
O7 Mo1 O10 89.22(19) 2_554 2
O10 Mo1 K1 46.44(13) 2 .
O10 Mo1 K3 48.35(13) 2 .
O10 Mo1 F9 76.86(17) 2 .
O10 Mo1 F10 0.0(3) 2 2
O17 Mo1 K1 126.51(19) . .
O17 Mo1 K3 126.3(2) . .
O17 Mo1 F4 100.4(2) . .
O17 Mo1 F5 99.9(2) . .
O17 Mo1 F7 98.3(2) . 2_554
O17 Mo1 F9 177.0(2) . .
O17 Mo1 F10 100.2(2) . 2
O17 Mo1 O7 98.3(2) . 2_554
O17 Mo1 O10 100.2(2) . 2
K4 Mo2 K1 69.81(4) 2_564 .
F6 Mo2 K1 45.52(14) . .
F6 Mo2 K4 46.84(14) . 2_564
F6 Mo2 F8 88.2(2) . 2_564
F6 Mo2 F9 79.25(18) . .
F6 Mo2 O8 88.2(2) . 2_564
F8 Mo2 K1 112.63(14) 2_564 .
F8 Mo2 K4 45.00(14) 2_564 2_564
F8 Mo2 F9 79.34(18) 2_564 .
F9 Mo2 K1 51.38(11) . .
F9 Mo2 K4 60.68(12) . 2_564
F11 Mo2 K1 52.71(15) . .
F11 Mo2 K4 122.40(15) . 2_564
F11 Mo2 F6 88.8(2) . .
F11 Mo2 F8 158.6(2) . 2_564
F11 Mo2 F9 79.27(18) . .
F11 Mo2 F12 89.2(2) . .
F11 Mo2 O8 158.6(2) . 2_564
F12 Mo2 K1 119.13(16) . .
F12 Mo2 K4 118.77(14) . 2_564
F12 Mo2 F6 158.6(2) . .
F12 Mo2 F8 85.9(2) . 2_564
F12 Mo2 F9 79.42(18) . .
F12 Mo2 O8 85.9(2) . 2_564
O8 Mo2 K1 112.63(14) 2_564 .
O8 Mo2 K4 45.00(14) 2_564 2_564
O8 Mo2 F8 0.0(3) 2_564 2_564
O8 Mo2 F9 79.34(18) 2_564 .
O16 Mo2 K1 129.53(19) . .
O16 Mo2 K4 118.2(2) . 2_564
O16 Mo2 F6 100.7(2) . .
O16 Mo2 F8 99.2(2) . 2_564
O16 Mo2 F9 178.5(2) . .
O16 Mo2 F11 102.2(2) . .
O16 Mo2 F12 100.6(2) . .
O16 Mo2 O8 99.2(2) . 2_564
K5 Mo3 K6 108.15(5) . 2
F2 Mo3 K5 43.78(14) 3_655 .
F2 Mo3 K5 43.78(14) . .
F2 Mo3 K6 110.70(15) 3_655 2
F2 Mo3 K6 110.70(15) . 2
F2 Mo3 F2 85.5(3) 3_655 .
F2 Mo3 F14 77.95(19) 3_655 1_545
F2 Mo3 F14 77.94(19) . 1_545
F13 Mo3 K5 121.86(19) . .
F13 Mo3 K5 121.87(19) 3_655 .
F13 Mo3 K6 54.74(17) 3_655 2
F13 Mo3 K6 54.74(17) . 2
F13 Mo3 F2 86.8(2) 3_655 .
F13 Mo3 F2 86.8(2) . 3_655
F13 Mo3 F2 159.2(2) . .
F13 Mo3 F2 159.2(2) 3_655 3_655
F13 Mo3 F13 93.7(4) 3_655 .
F13 Mo3 F14 81.6(2) 3_655 1_545
F13 Mo3 F14 81.6(2) . 1_545
F13 Mo3 O2 159.2(2) 3_655 3_655
F13 Mo3 O2 86.8(2) . 3_655
F14 Mo3 K5 62.86(17) 1_545 .
F14 Mo3 K6 45.29(17) 1_545 2
O2 Mo3 K5 43.78(14) 3_655 .
O2 Mo3 K6 110.70(15) 3_655 2
O2 Mo3 F2 85.5(3) 3_655 .
O2 Mo3 F2 0.0(3) 3_655 3_655
O2 Mo3 F14 77.95(19) 3_655 1_545
O13 Mo3 K5 121.87(19) 3_655 .
O13 Mo3 K6 54.74(17) 3_655 2
O13 Mo3 F2 86.8(2) 3_655 .
O13 Mo3 F2 159.2(2) 3_655 3_655
O13 Mo3 F13 93.7(4) 3_655 .
O13 Mo3 F13 0.0(4) 3_655 3_655
O13 Mo3 F14 81.6(2) 3_655 1_545
O13 Mo3 O2 159.2(2) 3_655 3_655
O18 Mo3 K5 112.9(3) . .
O18 Mo3 K6 139.0(3) . 2
O18 Mo3 F2 99.0(2) . 3_655
O18 Mo3 F2 99.0(2) . .
O18 Mo3 F13 101.2(2) . 3_655
O18 Mo3 F13 101.2(2) . .
O18 Mo3 F14 175.8(3) . 1_545
O18 Mo3 O2 99.0(2) . 3_655
O18 Mo3 O13 101.2(2) . 3_655
K6 Mo4 K2 67.85(3) 2_565 4_565
F1 Mo4 K2 49.26(14) 3_655 4_565
F1 Mo4 K2 121.44(15) . 4_565
F1 Mo4 K6 115.30(14) . 2_565
F1 Mo4 K6 115.30(14) 3_655 2_565
F1 Mo4 F1 89.1(3) . 3_655
F1 Mo4 F3 161.38(19) . 3_655
F1 Mo4 F3 87.46(18) 3_655 3_655
F1 Mo4 F3 161.38(19) 3_655 .
F1 Mo4 F3 87.46(18) . .
F1 Mo4 F14 82.26(19) . .
F1 Mo4 F14 82.26(19) 3_655 .
F1 Mo4 O1 89.1(3) . 3_655
F1 Mo4 O3 161.38(19) . 3_655
F1 Mo4 O3 87.46(18) 3_655 3_655
F3 Mo4 K2 118.68(13) . 4_565
F3 Mo4 K2 45.37(12) 3_655 4_565
F3 Mo4 K6 50.84(13) . 2_565
F3 Mo4 K6 50.84(13) 3_655 2_565
F3 Mo4 F3 89.9(2) 3_655 .
F3 Mo4 F14 79.14(17) . .
F3 Mo4 F14 79.14(17) 3_655 .
F14 Mo4 K2 56.78(2) . 4_565
F14 Mo4 K6 47.75(17) . 2_565
O1 Mo4 K2 49.26(14) 3_655 4_565
O1 Mo4 K6 115.30(14) 3_655 2_565
O1 Mo4 F1 0.0(4) 3_655 3_655
O1 Mo4 F3 87.46(18) 3_655 3_655
O1 Mo4 F3 161.38(19) 3_655 .
O1 Mo4 F14 82.26(19) 3_655 .
O1 Mo4 O3 87.46(18) 3_655 3_655
O3 Mo4 K2 45.37(12) 3_655 4_565
O3 Mo4 K6 50.84(13) 3_655 2_565
O3 Mo4 F3 0.0(3) 3_655 3_655
O3 Mo4 F3 89.9(2) 3_655 .
O3 Mo4 F14 79.14(17) 3_655 .
O19 Mo4 K2 123.13(3) . 4_565
O19 Mo4 K6 129.5(3) . 2_565
O19 Mo4 F1 99.7(2) . .
O19 Mo4 F1 99.7(2) . 3_655
O19 Mo4 F3 98.9(2) . .
O19 Mo4 F3 98.9(2) . 3_655
O19 Mo4 F14 177.2(3) . .
O19 Mo4 O1 99.7(2) . 3_655
O19 Mo4 O3 98.9(2) . 3_655
F2 K1 F3 76.00(14) 3_655 .
F2 K1 F6 134.71(16) 3_655 .
F2 K1 F7 81.85(15) 3_655 .
F2 K1 F8 132.07(16) 3_655 .
F2 K1 F10 76.89(15) 3_655 2
F2 K1 O10 76.89(15) 3_655 2
F3 K1 F6 74.65(13) . .
F3 K1 F7 126.62(14) . .
F3 K1 F10 140.71(14) . 2
F3 K1 O10 140.71(14) . 2
F6 K1 F7 143.41(14) . .
F6 K1 F10 106.51(14) . 2
F6 K1 O10 106.51(14) . 2
F7 K1 F10 76.23(13) . 2
F7 K1 O10 76.23(13) . 2
F8 K1 F3 84.77(14) . .
F8 K1 F6 78.17(15) . .
F8 K1 F7 75.28(15) . .
F8 K1 F10 134.44(15) . 2
F8 K1 O10 134.44(15) . 2
O2 K1 F2 0.0(3) 3_655 3_655
O2 K1 F3 76.00(14) 3_655 .
O2 K1 F6 134.71(16) 3_655 .
O2 K1 F7 81.85(15) 3_655 .
O2 K1 F8 132.07(16) 3_655 .
O2 K1 F10 76.89(15) 3_655 2
O2 K1 O10 76.89(15) 3_655 2
O10 K1 F10 0.0(3) 2 2
F3 K2 F1 54.98(12) 2_564 2_564
F3 K2 F7 148.42(14) 2_564 2_554
F3 K2 F12 67.78(14) 2_564 .
F3 K2 O1 54.98(12) 2_564 2_564
F3 K2 O7 148.42(14) 2_564 2_554
F6 K2 F1 68.57(14) 2_564 2_564
F6 K2 F3 75.24(14) 2_564 2_564
F6 K2 F7 131.76(14) 2_564 2_554
F6 K2 F12 117.60(15) 2_564 .
F6 K2 O1 68.57(14) 2_564 2_564
F6 K2 O3 75.24(14) 2_564 2_564
F6 K2 O7 131.76(14) 2_564 2_554
F7 K2 F1 141.69(13) 2_554 2_564
F7 K2 O1 141.69(13) 2_554 2_564
F10 K2 F1 79.23(13) . 2_564
F10 K2 F3 131.60(14) . 2_564
F10 K2 F6 73.95(14) . 2_564
F10 K2 F7 77.93(13) . 2_554
F10 K2 F12 160.61(15) . .
F10 K2 O1 79.23(13) . 2_564
F10 K2 O3 131.60(14) . 2_564
F10 K2 O6 73.95(14) . 2_564
F10 K2 O7 77.93(13) . 2_554
F12 K2 F1 118.86(13) . 2_564
F12 K2 F7 83.02(14) . 2_554
F12 K2 O1 118.86(13) . 2_564
F12 K2 O7 83.02(14) . 2_554
O1 K2 F1 0.00(18) 2_564 2_564
O3 K2 F1 54.98(12) 2_564 2_564
O3 K2 F3 0.0(2) 2_564 2_564
O3 K2 F7 148.42(14) 2_564 2_554
O3 K2 F12 67.78(14) 2_564 .
O3 K2 O1 54.98(12) 2_564 2_564
O3 K2 O7 148.42(14) 2_564 2_554
O6 K2 F1 68.57(14) 2_564 2_564
O6 K2 F3 75.24(14) 2_564 2_564
O6 K2 F6 0.0(3) 2_564 2_564
O6 K2 F7 131.76(14) 2_564 2_554
O6 K2 F12 117.60(15) 2_564 .
O6 K2 O1 68.57(14) 2_564 2_564
O6 K2 O3 75.24(14) 2_564 2_564
O6 K2 O7 131.76(14) 2_564 2_554
O7 K2 F1 141.69(13) 2_554 2_564
O7 K2 F7 0.0(3) 2_554 2_554
O7 K2 O1 141.69(13) 2_554 2_564
F7 K3 F5 113.20(14) 2_554 2
F7 K3 F9 55.34(12) 2_554 .
F7 K3 F11 108.85(13) 2_554 .
F7 K3 O5 113.20(14) 2_554 2
F9 K3 F5 116.42(13) . 2
F9 K3 O5 116.42(13) . 2
F10 K3 F5 68.20(13) 2 2
F10 K3 F7 57.68(13) 2 2_554
F10 K3 F9 53.69(12) 2 .
F10 K3 F11 87.41(14) 2 .
F10 K3 O5 68.20(13) 2 2
F10 K3 O7 57.68(13) 2 2_554
F11 K3 F5 104.45(14) . 2
F11 K3 F9 54.14(12) . .
F11 K3 O5 104.45(14) . 2
F13 K3 F5 145.91(16) 2_554 2
F13 K3 F7 67.82(16) 2_554 2_554
F13 K3 F9 92.66(15) 2_554 .
F13 K3 F10 125.34(17) 2_554 2
F13 K3 F11 107.14(15) 2_554 .
F13 K3 O5 145.91(16) 2_554 2
F13 K3 O7 67.82(16) 2_554 2_554
F13 K3 O10 125.34(17) 2_554 2
F13 K3 O16 90.02(16) 2_554 1_545
O5 K3 F5 0.00(15) 2 2
O7 K3 F5 113.20(14) 2_554 2
O7 K3 F7 0.0(3) 2_554 2_554
O7 K3 F9 55.34(12) 2_554 .
O7 K3 F11 108.85(13) 2_554 .
O7 K3 O5 113.20(14) 2_554 2
O10 K3 F5 68.20(13) 2 2
O10 K3 F7 57.68(13) 2 2_554
O10 K3 F9 53.69(12) 2 .
O10 K3 F10 0.0(3) 2 2
O10 K3 F11 87.41(14) 2 .
O10 K3 O5 68.20(13) 2 2
O10 K3 O7 57.68(13) 2 2_554
O13 K3 F5 145.91(16) 2_554 2
O13 K3 F7 67.82(16) 2_554 2_554
O13 K3 F9 92.66(15) 2_554 .
O13 K3 F10 125.34(17) 2_554 2
O13 K3 F11 107.14(15) 2_554 .
O13 K3 F13 0.0(3) 2_554 2_554
O13 K3 O5 145.91(16) 2_554 2
O13 K3 O7 67.82(16) 2_554 2_554
O13 K3 O10 125.34(17) 2_554 2
O13 K3 O16 90.02(16) 2_554 1_545
O16 K3 F5 61.80(15) 1_545 2
O16 K3 F7 68.27(15) 1_545 2_554
O16 K3 F9 117.07(15) 1_545 .
O16 K3 F10 74.61(15) 1_545 2
O16 K3 F11 160.35(16) 1_545 .
O16 K3 O5 61.80(15) 1_545 2
O16 K3 O7 68.27(15) 1_545 2_554
O16 K3 O10 74.61(15) 1_545 2
F1 K4 O5 153.80(14) 2_565 2_565
F4 K4 F1 99.58(13) 2_565 2_565
F4 K4 O1 99.58(13) 2_565 2_565
F4 K4 O5 54.33(12) 2_565 2_565
F4 K4 O17 157.82(15) 2_565 2
F6 K4 F1 68.47(13) 2_565 2_565
F6 K4 F4 79.73(14) 2_565 2_565
F6 K4 O1 68.47(13) 2_565 2_565
F6 K4 O4 79.73(14) 2_565 2_565
F6 K4 O5 100.94(14) 2_565 2_565
F6 K4 O17 80.66(15) 2_565 2
F8 K4 F1 117.47(15) . 2_565
F8 K4 F4 101.70(14) . 2_565
F8 K4 F6 58.88(14) . 2_565
F8 K4 O1 117.47(15) . 2_565
F8 K4 O4 101.70(14) . 2_565
F8 K4 O5 71.35(14) . 2_565
F8 K4 O6 58.88(14) . 2_565
F8 K4 O17 76.62(16) . 2
F11 K4 F1 126.70(14) . 2_565
F11 K4 F4 133.16(14) . 2_565
F11 K4 F6 120.60(16) . 2_565
F11 K4 F8 65.78(14) . .
F11 K4 O1 126.70(14) . 2_565
F11 K4 O4 133.16(14) . 2_565
F11 K4 O5 79.47(14) . 2_565
F11 K4 O6 120.60(16) . 2_565
F11 K4 O17 66.87(15) . 2
O1 K4 F1 0.0(2) 2_565 2_565
O1 K4 O5 153.80(14) 2_565 2_565
O4 K4 F1 99.58(13) 2_565 2_565
O4 K4 F4 0.0(2) 2_565 2_565
O4 K4 O1 99.58(13) 2_565 2_565
O4 K4 O5 54.33(12) 2_565 2_565
O4 K4 O17 157.82(15) 2_565 2
O6 K4 F1 68.47(13) 2_565 2_565
O6 K4 F4 79.73(14) 2_565 2_565
O6 K4 F6 0.0(2) 2_565 2_565
O6 K4 O1 68.47(13) 2_565 2_565
O6 K4 O4 79.73(14) 2_565 2_565
O6 K4 O5 100.94(14) 2_565 2_565
O6 K4 O17 80.66(15) 2_565 2
O17 K4 F1 63.33(15) 2 2_565
O17 K4 O1 63.33(15) 2 2_565
O17 K4 O5 140.73(16) 2 2_565
F1 K5 F1 55.26(18) 1_545 3_645
F1 K5 O1 55.26(18) 1_545 3_645
F2 K5 F1 100.05(15) . 1_545
F2 K5 F1 73.48(15) 3_655 1_545
F2 K5 F1 100.05(15) 3_655 3_645
F2 K5 F1 73.48(15) . 3_645
F2 K5 F2 59.3(2) . 3_655
F2 K5 F4 67.34(13) . 3_655
F2 K5 F4 67.34(13) 3_655 .
F2 K5 F4 120.61(15) 3_655 3_655
F2 K5 F4 120.62(15) . .
F2 K5 O1 100.05(15) . 1_545
F2 K5 O1 73.48(15) 3_655 1_545
F2 K5 O1 73.48(15) . 3_645
F2 K5 O1 100.05(15) 3_655 3_645
F2 K5 O2 59.3(2) . 3_655
F2 K5 O4 120.61(15) 3_655 3_655
F2 K5 O4 67.34(13) . 3_655
F4 K5 F1 142.77(13) . 3_645
F4 K5 F1 87.57(13) . 1_545
F4 K5 F1 142.77(13) 3_655 1_545
F4 K5 F1 87.57(13) 3_655 3_645
F4 K5 F4 129.40(19) . 3_655
F4 K5 O1 87.57(13) . 1_545
F4 K5 O1 87.57(13) 3_655 3_645
F4 K5 O1 142.77(13) . 3_645
F4 K5 O1 142.77(13) 3_655 1_545
F4 K5 O4 129.40(19) . 3_655
O1 K5 F1 0.00(18) 3_645 3_645
O1 K5 F1 55.26(18) 1_545 3_645
O1 K5 F1 0.00(18) 1_545 1_545
O1 K5 O1 55.26(18) 1_545 3_645
O2 K5 F1 100.05(15) 3_655 3_645
O2 K5 F1 73.48(15) 3_655 1_545
O2 K5 F2 0.0(3) 3_655 3_655
O2 K5 F4 67.34(13) 3_655 .
O2 K5 F4 120.61(15) 3_655 3_655
O2 K5 O1 73.48(15) 3_655 1_545
O2 K5 O1 100.05(15) 3_655 3_645
O2 K5 O4 120.61(15) 3_655 3_655
O4 K5 F1 87.57(13) 3_655 3_645
O4 K5 F1 142.77(13) 3_655 1_545
O4 K5 F4 0.0(2) 3_655 3_655
O4 K5 O1 87.57(13) 3_655 3_645
O4 K5 O1 142.77(13) 3_655 1_545
F3 K6 F3 57.37(17) 4_464 2_564
F3 K6 F13 110.48(15) 2_564 4_454
F3 K6 F13 86.16(15) 4_464 4_454
F3 K6 O3 57.37(17) 4_464 2_564
F3 K6 O13 86.16(15) 4_464 4_454
F3 K6 O13 110.48(15) 2_564 4_454
F12 K6 F3 126.72(16) 3 2_564
F12 K6 F3 126.73(16) . 4_464
F12 K6 F3 69.84(14) 3 4_464
F12 K6 F3 69.84(14) . 2_564
F12 K6 F12 158.2(3) . 3
F12 K6 F13 107.11(16) . 4_454
F12 K6 F13 56.05(15) 3 4_454
F12 K6 F14 89.75(12) 3 2_564
F12 K6 F14 89.76(12) . 2_564
F12 K6 O3 69.84(14) . 2_564
F12 K6 O3 69.84(14) 3 4_464
F12 K6 O3 126.72(16) 3 2_564
F12 K6 O3 126.73(16) . 4_464
F12 K6 O12 158.2(3) . 3
F12 K6 O13 56.05(15) 3 4_454
F12 K6 O13 107.11(16) . 4_454
F12 K6 O18 99.95(12) 3 2_564
F12 K6 O18 99.95(12) . 2_564
F14 K6 F3 56.43(13) 2_564 2_564
F14 K6 F3 56.43(13) 2_564 4_464
F14 K6 F13 54.10(15) 2_564 4_454
F14 K6 O3 56.43(13) 2_564 4_464
F14 K6 O3 56.43(13) 2_564 2_564
F14 K6 O13 54.10(15) 2_564 4_454
O3 K6 F3 0.0(2) 4_464 4_464
O3 K6 F3 57.37(17) 4_464 2_564
O3 K6 F3 0.0(2) 2_564 2_564
O3 K6 F13 86.16(15) 4_464 4_454
O3 K6 F13 110.48(15) 2_564 4_454
O3 K6 O3 57.37(17) 4_464 2_564
O3 K6 O13 86.16(15) 4_464 4_454
O3 K6 O13 110.48(15) 2_564 4_454
O12 K6 F3 69.84(14) 3 4_464
O12 K6 F3 126.72(16) 3 2_564
O12 K6 F12 0.0(2) 3 3
O12 K6 F13 56.05(15) 3 4_454
O12 K6 F14 89.75(12) 3 2_564
O12 K6 O3 69.84(14) 3 4_464
O12 K6 O3 126.72(16) 3 2_564
O12 K6 O13 56.05(15) 3 4_454
O12 K6 O18 99.95(12) 3 2_564
O13 K6 F13 0.0(3) 4_454 4_454
O18 K6 F3 67.89(17) 2_564 4_464
O18 K6 F3 67.89(17) 2_564 2_564
O18 K6 F13 150.42(14) 2_564 4_454
O18 K6 F14 115.5(2) 2_564 2_564
O18 K6 O3 67.89(17) 2_564 4_464
O18 K6 O3 67.89(17) 2_564 2_564
O18 K6 O13 150.42(14) 2_564 4_454
Mo4 F1 K2 101.36(18) . 2_565
Mo4 F1 K4 109.3(2) . 2_564
Mo4 F1 K5 103.87(18) . 1_565
K4 F1 K2 106.53(15) 2_564 2_565
K5 F1 K2 106.70(16) 1_565 2_565
K5 F1 K4 126.40(17) 1_565 2_564
Mo3 F2 K1 129.5(2) . 3_655
Mo3 F2 K2 102.68(19) . 4
Mo3 F2 K5 105.93(19) . .
K1 F2 K2 87.55(14) 3_655 4
K1 F2 K5 116.85(18) 3_655 .
K5 F2 K2 109.63(17) . 4
Mo4 F3 K1 134.3(2) . .
Mo4 F3 K2 105.19(16) . 2_565
Mo4 F3 K6 97.38(15) . 2_565
K1 F3 K2 90.22(12) . 2_565
K1 F3 K6 124.47(16) . 2_565
K2 F3 K6 94.69(13) 2_565 2_565
Mo1 F4 K1 101.51(16) . .
Mo1 F4 K4 105.66(17) . 2_564
Mo1 F4 K5 120.4(2) . .
K4 F4 K1 97.85(14) 2_564 .
K5 F4 K1 106.70(14) . .
K5 F4 K4 120.54(15) . 2_564
Mo1 F5 K2 102.36(18) . .
Mo1 F5 K3 106.1(2) . 2_554
Mo1 F5 K4 100.52(18) . 2_564
K2 F5 K4 108.96(15) . 2_564
K3 F5 K2 106.51(15) 2_554 .
K3 F5 K4 129.15(16) 2_554 2_564
Mo2 F6 K1 104.99(18) . .
Mo2 F6 K2 134.7(2) . 2_565
Mo2 F6 K4 102.66(18) . 2_564
K2 F6 K1 90.76(14) 2_565 .
K2 F6 K4 115.97(17) 2_565 2_564
K4 F6 K1 100.72(16) 2_564 .
Mo1 F7 K1 129.0(2) 2 .
Mo1 F7 K2 106.48(18) 2 2
Mo1 F7 K3 99.02(16) 2 2
K1 F7 K3 126.95(17) . 2
K2 F7 K1 87.79(13) 2 .
K2 F7 K3 100.11(15) 2 2
Mo2 F8 K1 129.0(2) 2_565 .
Mo2 F8 K2 99.73(18) 2_565 2_565
Mo2 F8 K4 104.54(18) 2_565 .
K1 F8 K2 85.35(13) . 2_565
K1 F8 K4 120.34(17) . .
K4 F8 K2 112.29(16) . 2_565
Mo1 F9 Mo2 168.3(2) . .
Mo1 F9 K1 93.30(14) . .
Mo1 F9 K2 84.59(12) . .
Mo1 F9 K3 92.92(15) . .
Mo1 F9 K4 87.23(14) . 2_564
Mo2 F9 K1 93.66(14) . .
Mo2 F9 K2 88.73(13) . .
Mo2 F9 K3 96.46(15) . .
Mo2 F9 K4 83.69(13) . 2_564
K1 F9 K2 177.18(15) . .
K1 F9 K4 87.10(12) . 2_564
K3 F9 K1 90.60(12) . .
K3 F9 K2 87.64(12) . .
K3 F9 K4 177.70(16) . 2_564
K4 F9 K2 94.66(11) 2_564 .
Mo1 F10 K1 103.19(16) 2_554 2_554
Mo1 F10 K2 139.2(2) 2_554 .
Mo1 F10 K3 100.12(17) 2_554 2_554
K2 F10 K1 89.73(13) . 2_554
K2 F10 K3 117.06(15) . 2_554
K3 F10 K1 95.77(14) 2_554 2_554
Mo2 F11 K1 97.48(17) . .
Mo2 F11 K3 104.09(18) . .
Mo2 F11 K4 130.3(2) . .
K3 F11 K1 89.49(14) . .
K4 F11 K1 107.55(15) . .
K4 F11 K3 117.99(16) . .
Mo2 F12 K2 113.6(2) . .
Mo2 F12 K3 96.24(18) . .
Mo2 F12 K6 134.8(2) . .
K2 F12 K3 94.99(15) . .
K6 F12 K2 100.57(15) . .
K6 F12 K3 109.82(17) . .
Mo3 F13 K2 106.0(2) . 2
Mo3 F13 K3 145.9(3) . 2
Mo3 F13 K6 96.2(2) . 2
K2 F13 K6 85.91(14) 2 2
K3 F13 K2 99.68(17) 2 2
K3 F13 K6 107.72(18) 2 2
Mo3 F14 K2 92.00(11) 1_565 4_565
Mo3 F14 K2 92.00(11) 1_565 2_565
Mo3 F14 K5 81.57(19) 1_565 1_565
Mo3 F14 K6 99.3(2) 1_565 2_565
Mo4 F14 Mo3 165.0(3) . 1_565
Mo4 F14 K2 88.14(11) . 4_565
Mo4 F14 K2 88.14(11) . 2_565
Mo4 F14 K5 83.5(2) . 1_565
Mo4 F14 K6 95.6(2) . 2_565
K2 F14 K2 176.0(2) 2_565 4_565
K2 F14 K5 90.59(12) 2_565 1_565
K2 F14 K5 90.59(12) 4_565 1_565
K6 F14 K2 89.38(12) 2_565 2_565
K6 F14 K2 89.38(12) 2_565 4_565
K6 F14 K5 179.1(2) 2_565 1_565
Mo2 O16 K3 157.4(3) . 1_565
Mo1 O17 K3 100.2(2) . 2_554
Mo1 O17 K4 147.6(3) . 2_554
K4 O17 K3 104.12(16) 2_554 2_554
Mo3 O18 K6 168.1(4) . 2_565
Mo4 O19 K4 97.9(2) . 4_564
Mo4 O19 K4 97.9(2) . 2_564
Mo4 O19 K5 145.1(4) . .
K4 O19 K4 111.4(2) 2_564 4_564
K5 O19 K4 101.51(16) . 4_564
K5 O19 K4 101.51(16) . 2_564
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
I2D I6D 3.007(3) 1_545
I2D I1D 1.788(4) .
I2D I3D 1.818(4) .
I2D I4D 2.959(3) .
I2D K3 3.7249(19) 2_565
I2D K3 3.7249(19) 4_565
I2D K4 3.778(2) 4_565
I2D K4 3.778(2) 2_565
I2D K5 3.886(3) 1_566
I2D K6 3.608(2) 2_565
I6D I2D 3.007(3) 1_565
I6D I1D 1.219(5) 1_565
I6D I3D 2.938(5) .
I6D I4D 1.795(4) .
I6D I5D 0.888(4) .
I6D K4 3.522(2) 4_575
I6D K4 3.522(2) 2_575
I6D K6 3.565(3) 2_575
I1D I6D 1.219(5) 1_545
I1D I4D 3.012(5) 1_545
I1D I5D 2.106(6) 1_545
I1D K4 3.315(2) 4_565
I1D K4 3.315(2) 2_565
I1D K6 3.263(4) 2_565
I3D I4D 1.145(5) .
I3D I5D 2.051(6) .
I3D K3 3.312(2) 4_565
I3D K3 3.312(2) 2_565
I3D K5 3.375(4) 1_566
I4D I1D 3.012(5) 1_565
I4D I5D 0.907(4) .
I4D K3 3.584(2) 4_565
I4D K3 3.584(2) 2_565
I4D K5 3.416(3) 1_566
I5D I1D 2.106(6) 1_565
I5D K3 4.003(3) 4_565
I5D K3 4.003(3) 2_565
I5D K4 3.890(3) 4_575
I5D K4 3.890(3) 2_575
I5D K5 3.761(4) 1_566
I5D K6 4.047(4) 2_575
Mo1 F4 1.928(4) .
Mo1 F5 1.858(5) .
Mo1 F7 1.925(4) 2_554
Mo1 F9 2.160(4) .
Mo1 F10 1.958(4) 2
Mo1 O7 1.925(4) 2_554
Mo1 O10 1.958(4) 2
Mo1 O17 1.667(5) .
Mo2 F6 1.933(4) .
Mo2 F8 1.946(4) 2_564
Mo2 F9 2.178(4) .
Mo2 F11 1.902(4) .
Mo2 F12 1.912(4) .
Mo2 O8 1.946(4) 2_564
Mo2 O16 1.663(5) .
Mo3 F2 1.966(4) 3_655
Mo3 F2 1.966(4) .
Mo3 F13 1.835(5) 3_655
Mo3 F13 1.835(5) .
Mo3 F14 2.203(6) 1_545
Mo3 O2 1.966(4) 3_655
Mo3 O13 1.835(5) 3_655
Mo3 O18 1.681(7) .
Mo4 F1 1.897(4) 3_655
Mo4 F1 1.897(4) .
Mo4 F3 1.931(4) .
Mo4 F3 1.931(4) 3_655
Mo4 F14 2.180(6) .
Mo4 O1 1.897(4) 3_655
Mo4 O3 1.931(4) 3_655
Mo4 O19 1.666(7) .
K1 F2 2.612(5) 3_655
K1 F3 2.749(4) .
K1 F6 2.802(5) .
K1 F7 2.805(4) .
K1 F8 2.622(4) .
K1 F10 2.807(5) 2
K1 O2 2.612(5) 3_655
K1 O10 2.807(5) 2
K2 F1 2.930(5) 2_564
K2 F3 2.796(4) 2_564
K2 F6 2.717(4) 2_564
K2 F7 2.803(5) 2_554
K2 F10 2.704(4) .
K2 F12 2.796(5) .
K2 O1 2.930(5) 2_564
K2 O3 2.796(4) 2_564
K2 O6 2.717(4) 2_564
K2 O7 2.803(5) 2_554
K3 F5 2.887(5) 2
K3 F7 2.855(5) 2_554
K3 F9 2.878(5) .
K3 F10 2.797(5) 2
K3 F11 2.859(5) .
K3 F13 2.668(5) 2_554
K3 O5 2.887(5) 2
K3 O7 2.855(5) 2_554
K3 O10 2.797(5) 2
K3 O13 2.668(5) 2_554
K3 O16 2.764(6) 1_545
K4 F1 2.884(5) 2_565
K4 F4 2.821(5) 2_565
K4 F6 2.778(5) 2_565
K4 F8 2.714(5) .
K4 F11 2.690(5) .
K4 O1 2.884(5) 2_565
K4 O4 2.821(5) 2_565
K4 O5 3.018(5) 2_565
K4 O6 2.778(5) 2_565
K4 O17 2.845(6) 2
K5 F1 2.870(5) 1_545
K5 F1 2.870(5) 3_645
K5 F2 2.696(5) .
K5 F2 2.696(5) 3_655
K5 F4 2.758(4) 3_655
K5 F4 2.758(4) .
K5 O1 2.870(5) 3_645
K5 O1 2.870(5) 1_545
K5 O2 2.696(5) 3_655
K5 O4 2.758(4) 3_655
K6 F3 2.843(5) 4_464
K6 F3 2.843(5) 2_564
K6 F12 2.592(4) 3
K6 F12 2.592(4) .
K6 F13 3.084(6) 4_454
K6 F14 2.704(7) 2_564
K6 O3 2.843(5) 2_564
K6 O3 2.843(5) 4_464
K6 O12 2.592(4) 3
K6 O13 3.084(6) 4_454
K6 O18 2.687(8) 2_564
F1 K2 2.930(5) 2_565
F1 K4 2.884(5) 2_564
F1 K5 2.870(5) 1_565
F2 K1 2.612(5) 3_655
F2 K2 2.994(5) 4
F3 K2 2.796(4) 2_565
F3 K6 2.843(5) 2_565
F4 K4 2.821(5) 2_564
F5 K3 2.887(5) 2_554
F5 K4 3.018(5) 2_564
F6 K2 2.717(4) 2_565
F6 K4 2.778(5) 2_564
F7 Mo1 1.925(4) 2
F7 K2 2.803(5) 2
F7 K3 2.855(5) 2
F8 Mo2 1.946(4) 2_565
F8 K2 3.145(5) 2_565
F9 K4 3.259(5) 2_564
F10 Mo1 1.958(4) 2_554
F10 K1 2.807(4) 2_554
F10 K3 2.797(5) 2_554
F13 K2 3.001(6) 2
F13 K3 2.668(5) 2
F13 K6 3.084(6) 2
F14 Mo3 2.203(6) 1_565
F14 K2 3.1732(16) 4_565
F14 K2 3.1732(16) 2_565
F14 K5 3.372(7) 1_565
F14 K6 2.704(7) 2_565
O16 K3 2.764(6) 1_565
O17 K3 3.181(6) 2_554
O17 K4 2.845(6) 2_554
O18 K6 2.687(8) 2_565
O19 K4 3.348(5) 2_564
O19 K4 3.348(5) 4_564
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
I1D I4D I5D I3D 180.00(3) 1_565 .
I1D I4D I5D K3 -115.15(14) 1_565 2_565
I1D I4D I5D K3 115.15(14) 1_565 4_565
I1D I4D I5D K4 54.85(18) 1_565 4_575
I1D I4D I5D K4 -54.85(17) 1_565 2_575
I1D I4D I5D K5 0.00(7) 1_565 1_566
I1D I4D I5D K6 180.00(7) 1_565 2_575
I3D I6D I4D I1D 180.00(4) . 1_565
I3D I6D I4D I5D 0.00(19) . .
I3D I6D I4D K3 -65.15(9) . 2_565
I3D I6D I4D K3 65.15(9) . 4_565
I3D I6D I4D K5 180.00(5) . 1_566
I3D I6D I5D I1D 180.0(7) . 1_565
I3D I6D I5D K3 -65.9(6) . 2_565
I3D I6D I5D K3 65.9(9) . 4_565
I3D I6D I5D K4 124.3(7) . 4_575
I3D I6D I5D K4 -124.3(8) . 2_575
I3D I6D I5D K5 180.0(8) . 1_566
I3D I6D I5D K6 0.0(8) . 2_575
I4D I2D I3D K3 114.03(7) . 4_565
I4D I2D I3D K3 -114.03(7) . 2_565
I4D I2D I3D K5 0.00(3) . 1_566
I4D I6D I3D I5D 0.0(9) . .
I4D I6D I3D K3 113.86(9) . 2_565
I4D I6D I3D K3 -113.86(9) . 4_565
I4D I6D I3D K5 0.00(5) . 1_566
I4D I6D I5D I1D 0.0(3) . 1_565
I4D I6D I5D K3 114.1(3) . 2_565
I4D I6D I5D K3 -114.1(3) . 4_565
I4D I6D I5D K4 55.7(2) . 2_575
I4D I6D I5D K4 -55.7(2) . 4_575
I4D I6D I5D K5 0.00(17) . 1_566
I4D I6D I5D K6 180.00(17) . 2_575
I4D I3D I5D K3 113.85(11) . 4_565
I4D I3D I5D K3 -113.85(11) . 2_565
I4D I3D I5D K4 -55.87(13) . 2_575
I4D I3D I5D K4 55.87(13) . 4_575
I4D I3D I5D K5 0.00(7) . 1_566
I4D I3D I5D K6 180.00(7) . 2_575
I5D I6D I3D I4D 0.0(5) . .
I5D I6D I3D K3 -113.9(5) . 4_565
I5D I6D I3D K3 113.9(5) . 2_565
I5D I6D I3D K5 0.0(5) . 1_566
I5D I6D I4D I1D 180.00(13) . 1_565
I5D I6D I4D K3 -65.15(16) . 2_565
I5D I6D I4D K3 65.15(16) . 4_565
I5D I6D I4D K5 180.00(14) . 1_566
I5D I3D I4D I2D 180.00(4) . .
I5D I3D I4D K3 -66.25(9) . 4_565
I5D I3D I4D K3 66.25(9) . 2_565
I5D I3D I4D K5 180.00(5) . 1_566
K1 Mo1 F4 K4 -101.64(19) . 2_564
K1 Mo1 F4 K5 117.4(3) . .
K1 Mo1 F5 K2 -96.98(14) . .
K1 Mo1 F5 K3 151.53(9) . 2_554
K1 Mo1 F5 K4 15.29(19) . 2_564
K1 Mo1 F9 Mo2 126.3(12) . .
K1 Mo1 F9 K2 -178.12(16) . .
K1 Mo1 F9 K3 -90.77(13) . .
K1 Mo1 F9 K4 86.93(12) . 2_564
K1 Mo1 O17 K3 -145.86(9) . 2_554
K1 Mo1 O17 K4 75.9(6) . 2_554
K1 Mo2 F6 K2 -106.5(3) . 2_565
K1 Mo2 F6 K4 104.9(2) . 2_564
K1 Mo2 F9 Mo1 -126.2(12) . .
K1 Mo2 F9 K2 178.50(17) . .
K1 Mo2 F9 K3 91.02(14) . .
K1 Mo2 F9 K4 -86.67(12) . 2_564
K1 Mo2 F11 K3 -91.36(18) . .
K1 Mo2 F11 K4 120.7(3) . .
K1 Mo2 F12 K2 -85.9(2) . .
K1 Mo2 F12 K3 12.30(18) . .
K1 Mo2 F12 K6 138.4(3) . .
K1 Mo2 O16 K3 59.2(9) . 1_565
K2 Mo4 F1 K2 -95.25(15) 4_565 2_565
K2 Mo4 F1 K4 152.56(9) 4_565 2_564
K2 Mo4 F1 K5 15.3(2) 4_565 1_565
K2 Mo4 F3 K1 -158.59(18) 4_565 .
K2 Mo4 F3 K2 95.73(15) 4_565 2_565
K2 Mo4 F3 K6 -1.20(17) 4_565 2_565
K2 Mo4 F14 Mo3 90.81(12) 4_565 1_565
K2 Mo4 F14 K2 -178.4(2) 4_565 2_565
K2 Mo4 F14 K5 90.81(11) 4_565 1_565
K2 Mo4 F14 K6 -89.19(11) 4_565 2_565
K2 Mo4 O19 K4 -149.14(6) 4_565 2_564
K2 Mo4 O19 K4 -36.1(3) 4_565 4_564
K2 Mo4 O19 K5 87.37(19) 4_565 .
K3 I2D I1D K4 173.56(5) 4_565 2_565
K3 I2D I1D K4 -60.47(9) 2_565 2_565
K3 I2D I1D K4 60.47(9) 4_565 4_565
K3 I2D I1D K4 -173.56(5) 2_565 4_565
K3 I2D I1D K6 62.99(5) 2_565 2_565
K3 I2D I1D K6 -62.99(5) 4_565 2_565
K3 I2D I3D K3 131.93(10) 4_565 2_565
K3 I2D I3D K5 -114.03(5) 4_565 1_566
K3 I2D I3D K5 114.03(5) 2_565 1_566
K3 I2D I4D I3D -64.94(4) 2_565 .
K3 I2D I4D I3D 64.94(4) 4_565 .
K3 I2D I4D K3 129.87(7) 4_565 2_565
K3 I2D I4D K3 -129.87(7) 2_565 4_565
K3 I2D I4D K5 -115.06(3) 4_565 1_566
K3 I2D I4D K5 115.06(3) 2_565 1_566
K3 I3D I4D I2D 113.75(7) 2_565 .
K3 I3D I4D I2D -113.75(7) 4_565 .
K3 I3D I4D K3 -132.50(12) 2_565 4_565
K3 I3D I4D K3 132.50(12) 4_565 2_565
K3 I3D I4D K5 113.75(6) 2_565 1_566
K3 I3D I4D K5 -113.75(6) 4_565 1_566
K3 I3D I5D I4D 113.85(8) 2_565 .
K3 I3D I5D K3 -132.29(11) 2_565 4_565
K3 I3D I5D K3 132.29(11) 4_565 2_565
K3 I3D I5D K4 169.73(8) 2_565 4_575
K3 I3D I5D K4 57.98(13) 2_565 2_575
K3 I3D I5D K4 -169.73(8) 4_565 2_575
K3 I3D I5D K4 -57.98(13) 4_565 4_575
K3 I3D I5D K5 -113.85(6) 4_565 1_566
K3 I3D I5D K5 113.85(6) 2_565 1_566
K3 I3D I5D K6 66.15(6) 4_565 2_575
K3 I3D I5D K6 -66.15(6) 2_565 2_575
K3 I4D I5D I3D -64.85(14) 2_565 .
K3 I4D I5D I3D 64.85(14) 4_565 .
K3 I4D I5D K3 -129.7(2) 2_565 4_565
K3 I4D I5D K3 129.7(2) 4_565 2_565
K3 I4D I5D K4 -170.01(7) 4_565 2_575
K3 I4D I5D K4 -60.3(2) 4_565 4_575
K3 I4D I5D K4 170.01(7) 2_565 4_575
K3 I4D I5D K4 60.3(2) 2_565 2_575
K3 I4D I5D K5 -115.15(10) 4_565 1_566
K3 I4D I5D K5 115.15(10) 2_565 1_566
K3 I4D I5D K6 -64.85(10) 2_565 2_575
K3 I4D I5D K6 64.85(10) 4_565 2_575
K3 Mo1 F4 K1 8.86(18) . .
K3 Mo1 F4 K4 -92.78(15) . 2_564
K3 Mo1 F4 K5 126.24(16) . .
K3 Mo1 F5 K2 -18.7(2) . .
K3 Mo1 F5 K3 -130.16(11) . 2_554
K3 Mo1 F5 K4 93.60(14) . 2_564
K3 Mo1 F9 Mo2 -143.0(12) . .
K3 Mo1 F9 K1 90.77(13) . .
K3 Mo1 F9 K2 -87.35(12) . .
K3 Mo1 F9 K4 177.70(16) . 2_564
K3 Mo1 O17 K3 126.49(13) . 2_554
K3 Mo1 O17 K4 -11.7(7) . 2_554
K4 I2D I1D K4 113.09(10) 4_565 2_565
K4 I2D I1D K4 -113.09(10) 2_565 4_565
K4 I2D I1D K6 -123.45(5) 4_565 2_565
K4 I2D I1D K6 123.45(5) 2_565 2_565
K4 I2D I3D K3 174.00(5) 2_565 4_565
K4 I2D I3D K3 54.07(11) 4_565 4_565
K4 I2D I3D K3 -174.00(5) 4_565 2_565
K4 I2D I3D K3 -54.07(11) 2_565 2_565
K4 I2D I3D K5 59.96(7) 2_565 1_566
K4 I2D I3D K5 -59.96(7) 4_565 1_566
K4 I2D I4D I3D -121.23(5) 2_565 .
K4 I2D I4D I3D 121.23(5) 4_565 .
K4 I2D I4D K3 173.84(5) 2_565 4_565
K4 I2D I4D K3 56.29(6) 4_565 4_565
K4 I2D I4D K3 -56.29(6) 2_565 2_565
K4 I2D I4D K3 -173.84(5) 4_565 2_565
K4 I2D I4D K5 58.77(4) 2_565 1_566
K4 I2D I4D K5 -58.77(4) 4_565 1_566
K4 I6D I3D I4D 55.75(7) 4_575 .
K4 I6D I3D I4D -55.75(7) 2_575 .
K4 I6D I3D I5D -55.8(9) 2_575 .
K4 I6D I3D I5D 55.8(9) 4_575 .
K4 I6D I3D K3 -58.11(9) 4_575 4_565
K4 I6D I3D K3 58.11(9) 2_575 2_565
K4 I6D I3D K3 169.61(6) 4_575 2_565
K4 I6D I3D K3 -169.61(6) 2_575 4_565
K4 I6D I3D K5 -55.75(5) 2_575 1_566
K4 I6D I3D K5 55.75(5) 4_575 1_566
K4 I6D I4D I1D -55.45(7) 2_575 1_565
K4 I6D I4D I1D 55.45(7) 4_575 1_565
K4 I6D I4D I5D 124.6(2) 2_575 .
K4 I6D I4D I5D -124.55(18) 4_575 .
K4 I6D I4D K3 -59.40(10) 4_575 4_565
K4 I6D I4D K3 -170.30(6) 2_575 4_565
K4 I6D I4D K3 59.40(10) 2_575 2_565
K4 I6D I4D K3 170.30(6) 4_575 2_565
K4 I6D I4D K5 55.45(5) 4_575 1_566
K4 I6D I4D K5 -55.45(5) 2_575 1_566
K4 I6D I5D I1D -55.68(15) 2_575 1_565
K4 I6D I5D I1D 55.68(14) 4_575 1_565
K4 I6D I5D K3 -169.78(12) 2_575 4_565
K4 I6D I5D K3 -58.4(3) 4_575 4_565
K4 I6D I5D K3 58.4(3) 2_575 2_565
K4 I6D I5D K3 169.78(12) 4_575 2_565
K4 I6D I5D K4 -111.36(17) 2_575 4_575
K4 I6D I5D K4 111.36(17) 4_575 2_575
K4 I6D I5D K5 55.68(9) 4_575 1_566
K4 I6D I5D K5 -55.68(9) 2_575 1_566
K4 I6D I5D K6 -124.32(9) 4_575 2_575
K4 I6D I5D K6 124.32(9) 2_575 2_575
K4 Mo2 F6 K1 -104.9(2) 2_564 .
K4 Mo2 F6 K2 148.6(4) 2_564 2_565
K4 Mo2 F9 Mo1 -39.6(11) 2_564 .
K4 Mo2 F9 K1 86.67(12) 2_564 .
K4 Mo2 F9 K2 -94.83(10) 2_564 .
K4 Mo2 F9 K3 177.69(16) 2_564 .
K4 Mo2 F11 K1 4.4(2) 2_564 .
K4 Mo2 F11 K3 -86.96(17) 2_564 .
K4 Mo2 F11 K4 125.1(2) 2_564 .
K4 Mo2 F12 K2 -4.3(3) 2_564 .
K4 Mo2 F12 K3 93.97(14) 2_564 .
K4 Mo2 F12 K6 -139.9(3) 2_564 .
K4 Mo2 O16 K3 -27.1(9) 2_564 1_565
K5 I2D I1D K4 -56.55(5) 1_566 4_565
K5 I2D I1D K4 56.55(5) 1_566 2_565
K5 I2D I1D K6 180.0 1_566 2_565
K5 I2D I3D K3 114.03(5) 1_566 4_565
K5 I2D I3D K3 -114.03(5) 1_566 2_565
K5 I2D I4D I3D 180.00(3) 1_566 .
K5 I2D I4D K3 -115.06(3) 1_566 2_565
K5 I2D I4D K3 115.06(3) 1_566 4_565
K5 I3D I4D I2D 0.00(2) 1_566 .
K5 I3D I4D K3 -113.75(6) 1_566 2_565
K5 I3D I4D K3 113.75(6) 1_566 4_565
K5 I3D I5D I4D 0.00(6) 1_566 .
K5 I3D I5D K3 -113.85(6) 1_566 2_565
K5 I3D I5D K3 113.85(6) 1_566 4_565
K5 I3D I5D K4 -55.87(9) 1_566 2_575
K5 I3D I5D K4 55.87(9) 1_566 4_575
K5 I3D I5D K6 180.000(1) 1_566 2_575
K5 I4D I5D I3D 180.00(7) 1_566 .
K5 I4D I5D K3 115.15(10) 1_566 4_565
K5 I4D I5D K3 -115.15(10) 1_566 2_565
K5 I4D I5D K4 -54.85(14) 1_566 2_575
K5 I4D I5D K4 54.85(14) 1_566 4_575
K5 I4D I5D K6 180.000(2) 1_566 2_575
K5 Mo3 F2 K1 147.6(4) . 3_655
K5 Mo3 F2 K2 -115.0(2) . 4
K5 Mo3 F13 K2 3.1(3) . 2
K5 Mo3 F13 K3 -134.4(4) . 2
K5 Mo3 F13 K6 90.56(18) . 2
K5 Mo3 O18 K6 0.000(4) . 2_565
K6 I2D I1D K4 -123.45(5) 2_565 2_565
K6 I2D I1D K4 123.45(5) 2_565 4_565
K6 I2D I3D K3 65.97(5) 2_565 2_565
K6 I2D I3D K3 -65.97(5) 2_565 4_565
K6 I2D I3D K5 180.0 2_565 1_566
K6 I2D I4D I3D 0.00(3) 2_565 .
K6 I2D I4D K3 64.94(3) 2_565 2_565
K6 I2D I4D K3 -64.94(3) 2_565 4_565
K6 I2D I4D K5 180.0 2_565 1_566
K6 I6D I3D I4D 180.00(5) 2_575 .
K6 I6D I3D I5D 180.0(9) 2_575 .
K6 I6D I3D K3 66.14(6) 2_575 4_565
K6 I6D I3D K3 -66.14(6) 2_575 2_565
K6 I6D I3D K5 180.0 2_575 1_566
K6 I6D I4D I1D 180.00(4) 2_575 1_565
K6 I6D I4D I5D 0.00(18) 2_575 .
K6 I6D I4D K3 65.15(6) 2_575 4_565
K6 I6D I4D K3 -65.15(6) 2_575 2_565
K6 I6D I4D K5 180.0 2_575 1_566
K6 I6D I5D I1D 180.00(9) 2_575 1_565
K6 I6D I5D K3 65.90(18) 2_575 4_565
K6 I6D I5D K3 -65.90(18) 2_575 2_565
K6 I6D I5D K4 -124.32(9) 2_575 2_575
K6 I6D I5D K4 124.32(9) 2_575 4_575
K6 I6D I5D K5 180.0 2_575 1_566
K6 Mo3 F2 K1 -117.4(3) 2 3_655
K6 Mo3 F2 K2 -20.00(18) 2 4
K6 Mo3 F2 K5 94.98(17) 2 .
K6 Mo3 F13 K2 -87.50(19) 2 2
K6 Mo3 F13 K3 135.0(6) 2 2
K6 Mo3 O18 K6 180.000(2) 2 2_565
K6 Mo4 F1 K2 -16.78(19) 2_565 2_565
K6 Mo4 F1 K4 -128.97(13) 2_565 2_564
K6 Mo4 F1 K5 93.80(15) 2_565 1_565
K6 Mo4 F3 K1 -157.4(3) 2_565 .
K6 Mo4 F3 K2 96.92(17) 2_565 2_565
K6 Mo4 F14 Mo3 180.000(3) 2_565 1_565
K6 Mo4 F14 K2 89.19(12) 2_565 4_565
K6 Mo4 F14 K2 -89.19(12) 2_565 2_565
K6 Mo4 F14 K5 180.0 2_565 1_565
K6 Mo4 O19 K4 -123.49(15) 2_565 4_564
K6 Mo4 O19 K4 123.49(15) 2_565 2_564
K6 Mo4 O19 K5 0.000(2) 2_565 .
F1 Mo4 F1 K2 -134.53(10) 3_655 2_565
F1 Mo4 F1 K4 113.28(16) 3_655 2_564
F1 Mo4 F1 K5 -23.9(3) 3_655 1_565
F1 Mo4 F3 K1 156.3(5) 3_655 .
F1 Mo4 F3 K1 76.6(3) . .
F1 Mo4 F3 K2 50.6(6) 3_655 2_565
F1 Mo4 F3 K2 -29.08(19) . 2_565
F1 Mo4 F3 K6 -46.3(6) 3_655 2_565
F1 Mo4 F3 K6 -126.00(17) . 2_565
F1 Mo4 F14 Mo3 -45.09(14) . 1_565
F1 Mo4 F14 Mo3 45.09(14) 3_655 1_565
F1 Mo4 F14 K2 135.90(19) 3_655 2_565
F1 Mo4 F14 K2 45.71(17) . 2_565
F1 Mo4 F14 K2 -135.90(19) . 4_565
F1 Mo4 F14 K2 -45.71(17) 3_655 4_565
F1 Mo4 F14 K5 45.09(14) 3_655 1_565
F1 Mo4 F14 K5 -45.09(14) . 1_565
F1 Mo4 F14 K6 134.91(14) . 2_565
F1 Mo4 F14 K6 -134.91(14) 3_655 2_565
F1 Mo4 O19 K4 101.90(18) . 4_564
F1 Mo4 O19 K4 -101.90(18) 3_655 2_564
F1 Mo4 O19 K4 -11.1(2) . 2_564
F1 Mo4 O19 K4 11.1(2) 3_655 4_564
F1 Mo4 O19 K5 134.60(14) 3_655 .
F1 Mo4 O19 K5 -134.60(14) . .
F1 K2 F5 Mo1 -150.06(18) 2_564 .
F1 K2 F5 K3 -38.9(3) 2_564 2_554
F1 K2 F5 K4 104.1(2) 2_564 2_564
F1 K2 F9 Mo1 -170.1(5) 2_564 .
F1 K2 F9 Mo2 0.2(6) 2_564 .
F1 K2 F9 K3 96.8(5) 2_564 .
F1 K2 F9 K4 -83.3(5) 2_564 2_564
F1 K2 F10 Mo1 0.1(3) 2_564 2_554
F1 K2 F10 K1 -110.00(14) 2_564 2_554
F1 K2 F10 K3 153.66(19) 2_564 2_554
F1 K2 F12 Mo2 -130.2(2) 2_564 .
F1 K2 F12 K3 130.78(14) 2_564 .
F1 K2 F12 K6 19.5(2) 2_564 .
F1 K4 F8 Mo2 -53.7(2) 2_565 2_565
F1 K4 F8 K1 101.2(2) 2_565 .
F1 K4 F8 K2 -160.81(13) 2_565 2_565
F1 K4 F11 Mo2 151.0(2) 2_565 .
F1 K4 F11 K1 -92.4(2) 2_565 .
F1 K4 F11 K3 6.6(3) 2_565 .
F1 K5 F2 Mo3 -50.8(2) 1_545 .
F1 K5 F2 Mo3 -99.8(2) 3_645 .
F1 K5 F2 K1 107.8(2) 3_645 3_655
F1 K5 F2 K1 156.77(19) 1_545 3_655
F1 K5 F2 K2 59.32(17) 1_545 4
F1 K5 F2 K2 10.32(13) 3_645 4
F1 K5 F4 Mo1 -27.1(4) 3_645 .
F1 K5 F4 Mo1 -30.3(2) 1_545 .
F1 K5 F4 K1 84.42(16) 1_545 .
F1 K5 F4 K1 87.6(3) 3_645 .
F1 K5 F4 K4 -162.3(2) 3_645 2_564
F1 K5 F4 K4 -165.54(18) 1_545 2_564
F1 K5 O19 Mo4 63.7(3) 1_545 .
F1 K5 O19 Mo4 -63.7(3) 3_645 .
F1 K5 O19 K4 58.9(4) 3_645 4_564
F1 K5 O19 K4 -58.9(4) 1_545 2_564
F1 K5 O19 K4 173.8(2) 3_645 2_564
F1 K5 O19 K4 -173.8(2) 1_545 4_564
F2 Mo3 F2 K1 132.2(2) 3_655 3_655
F2 Mo3 F2 K2 -130.43(12) 3_655 4
F2 Mo3 F2 K5 -15.4(3) 3_655 .
F2 Mo3 F13 K2 -37.6(8) . 2
F2 Mo3 F13 K2 30.7(2) 3_655 2
F2 Mo3 F13 K3 -106.8(5) 3_655 2
F2 Mo3 F13 K3 -175.1(4) . 2
F2 Mo3 F13 K6 49.9(7) . 2
F2 Mo3 F13 K6 118.2(2) 3_655 2
F2 Mo3 O18 K6 -43.39(15) 3_655 2_565
F2 Mo3 O18 K6 43.39(15) . 2_565
F2 K1 F3 Mo4 72.0(3) 3_655 .
F2 K1 F3 K2 -176.29(15) 3_655 2_565
F2 K1 F3 K6 -80.45(19) 3_655 2_565
F2 K1 F4 Mo1 115.2(2) 3_655 .
F2 K1 F4 K4 -136.99(18) 3_655 2_564
F2 K1 F4 K5 -11.75(15) 3_655 .
F2 K1 F6 Mo2 131.7(2) 3_655 .
F2 K1 F6 K2 -91.3(2) 3_655 2_565
F2 K1 F6 K4 25.3(3) 3_655 2_564
F2 K1 F7 Mo1 -150.2(3) 3_655 2
F2 K1 F7 K2 -40.70(14) 3_655 2
F2 K1 F7 K3 60.3(2) 3_655 2
F2 K1 F8 Mo2 2.5(4) 3_655 2_565
F2 K1 F8 K2 101.2(2) 3_655 2_565
F2 K1 F8 K4 -145.6(2) 3_655 .
F2 K1 F9 Mo1 9.8(2) 3_655 .
F2 K1 F9 Mo2 -160.72(16) 3_655 .
F2 K1 F9 K3 102.77(16) 3_655 .
F2 K1 F9 K4 -77.24(16) 3_655 2_564
F2 K1 F11 Mo2 -99.6(4) 3_655 .
F2 K1 F11 K3 4.6(5) 3_655 .
F2 K1 F11 K4 123.9(4) 3_655 .
F2 K5 F2 Mo3 13.0(2) 3_655 .
F2 K5 F2 K1 -139.40(14) 3_655 3_655
F2 K5 F2 K2 123.14(11) 3_655 4
F2 K5 F4 Mo1 -130.5(2) . .
F2 K5 F4 Mo1 -103.4(2) 3_655 .
F2 K5 F4 K1 -15.8(2) . .
F2 K5 F4 K1 11.32(14) 3_655 .
F2 K5 F4 K4 94.2(2) . 2_564
F2 K5 F4 K4 121.4(2) 3_655 2_564
F2 K5 O19 Mo4 30.10(10) 3_655 .
F2 K5 O19 Mo4 -30.10(10) . .
F2 K5 O19 K4 -92.45(17) 3_655 2_564
F2 K5 O19 K4 152.65(19) 3_655 4_564
F2 K5 O19 K4 -152.65(19) . 2_564
F2 K5 O19 K4 92.45(17) . 4_564
F3 Mo4 F1 K2 -55.1(6) 3_655 2_565
F3 Mo4 F1 K2 27.16(17) . 2_565
F3 Mo4 F1 K4 -85.04(19) . 2_564
F3 Mo4 F1 K4 -167.3(5) 3_655 2_564
F3 Mo4 F1 K5 55.5(6) 3_655 1_565
F3 Mo4 F1 K5 137.74(19) . 1_565
F3 Mo4 F3 K1 -121.8(2) 3_655 .
F3 Mo4 F3 K2 132.48(10) 3_655 2_565
F3 Mo4 F3 K6 35.6(2) 3_655 2_565
F3 Mo4 F14 Mo3 133.97(13) 3_655 1_565
F3 Mo4 F14 Mo3 -133.97(13) . 1_565
F3 Mo4 F14 K2 43.17(16) 3_655 4_565
F3 Mo4 F14 K2 -43.17(16) . 2_565
F3 Mo4 F14 K2 -135.22(19) 3_655 2_565
F3 Mo4 F14 K2 135.22(19) . 4_565
F3 Mo4 F14 K5 133.97(13) 3_655 1_565
F3 Mo4 F14 K5 -133.97(13) . 1_565
F3 Mo4 F14 K6 -46.03(13) 3_655 2_565
F3 Mo4 F14 K6 46.03(13) . 2_565
F3 Mo4 O19 K4 77.8(2) . 2_564
F3 Mo4 O19 K4 -169.17(17) . 4_564
F3 Mo4 O19 K4 -77.8(2) 3_655 4_564
F3 Mo4 O19 K4 169.17(17) 3_655 2_564
F3 Mo4 O19 K5 -45.68(13) . .
F3 Mo4 O19 K5 45.68(13) 3_655 .
F3 K1 F4 Mo1 -169.01(17) . .
F3 K1 F4 K4 -61.19(13) . 2_564
F3 K1 F4 K5 64.05(15) . .
F3 K1 F6 Mo2 -177.0(2) . .
F3 K1 F6 K2 -39.94(13) . 2_565
F3 K1 F6 K4 76.68(15) . 2_564
F3 K1 F7 Mo1 144.0(2) . 2
F3 K1 F7 K2 -106.44(16) . 2
F3 K1 F7 K3 -5.4(3) . 2
F3 K1 F8 Mo2 -63.3(3) . 2_565
F3 K1 F8 K2 35.43(12) . 2_565
F3 K1 F8 K4 148.6(2) . .
F3 K1 F9 Mo1 97.36(16) . .
F3 K1 F9 Mo2 -73.17(18) . .
F3 K1 F9 K3 -169.68(12) . .
F3 K1 F9 K4 10.31(15) . 2_564
F3 K1 F11 Mo2 58.2(2) . .
F3 K1 F11 K3 162.35(13) . .
F3 K1 F11 K4 -78.35(19) . .
F3 K2 F5 Mo1 120.8(2) 2_564 .
F3 K2 F5 K3 -127.95(19) 2_564 2_554
F3 K2 F5 K4 15.0(3) 2_564 2_564
F3 K2 F9 Mo1 -173.32(13) 2_564 .
F3 K2 F9 Mo2 -3.00(17) 2_564 .
F3 K2 F9 K3 93.52(13) 2_564 .
F3 K2 F9 K4 -86.56(13) 2_564 2_564
F3 K2 F10 Mo1 -18.1(4) 2_564 2_554
F3 K2 F10 K1 -128.18(15) 2_564 2_554
F3 K2 F10 K3 135.48(17) 2_564 2_554
F3 K2 F12 Mo2 -109.1(3) 2_564 .
F3 K2 F12 K3 151.87(15) 2_564 .
F3 K2 F12 K6 40.61(15) 2_564 .
F3 K6 F12 Mo2 100.2(4) 2_564 .
F3 K6 F12 Mo2 108.1(3) 4_464 .
F3 K6 F12 K2 -39.15(14) 2_564 .
F3 K6 F12 K2 -31.3(2) 4_464 .
F3 K6 F12 K3 -138.43(18) 2_564 .
F3 K6 F12 K3 -130.53(16) 4_464 .
F4 Mo1 F5 K2 -137.80(18) . .
F4 Mo1 F5 K3 110.71(19) . 2_554
F4 Mo1 F5 K4 -25.53(17) . 2_564
F4 Mo1 F9 Mo2 82.3(11) . .
F4 Mo1 F9 K1 -43.94(15) . .
F4 Mo1 F9 K2 137.95(15) . .
F4 Mo1 F9 K3 -134.71(17) . .
F4 Mo1 F9 K4 42.99(14) . 2_564
F4 Mo1 O17 K3 -100.58(19) . 2_554
F4 Mo1 O17 K4 121.2(5) . 2_554
F4 K4 F8 Mo2 53.8(2) 2_565 2_565
F4 K4 F8 K1 -151.4(2) 2_565 .
F4 K4 F8 K2 -53.40(17) 2_565 2_565
F4 K4 F11 Mo2 -18.5(4) 2_565 .
F4 K4 F11 K1 98.0(2) 2_565 .
F4 K4 F11 K3 -162.89(16) 2_565 .
F4 K5 F2 Mo3 42.3(3) . .
F4 K5 F2 Mo3 165.8(2) 3_655 .
F4 K5 F2 K1 13.43(17) 3_655 3_655
F4 K5 F2 K1 -110.1(2) . 3_655
F4 K5 F2 K2 152.46(15) . 4
F4 K5 F2 K2 -84.02(16) 3_655 4
F4 K5 F4 Mo1 144.82(14) 3_655 .
F4 K5 F4 K1 -100.5(2) 3_655 .
F4 K5 F4 K4 9.6(4) 3_655 2_564
F4 K5 O19 Mo4 99.41(12) . .
F4 K5 O19 Mo4 -99.41(12) 3_655 .
F4 K5 O19 K4 -138.0(2) . 4_564
F4 K5 O19 K4 23.14(14) 3_655 4_564
F4 K5 O19 K4 -23.14(14) . 2_564
F4 K5 O19 K4 138.0(2) 3_655 2_564
F5 Mo1 F4 K1 129.73(18) . .
F5 Mo1 F4 K4 28.09(19) . 2_564
F5 Mo1 F4 K5 -112.9(2) . .
F5 Mo1 F9 Mo2 -8.6(11) . .
F5 Mo1 F9 K1 -134.88(18) . .
F5 Mo1 F9 K2 47.00(15) . .
F5 Mo1 F9 K3 134.35(17) . .
F5 Mo1 F9 K4 -47.95(16) . 2_564
F5 Mo1 O17 K3 -9.0(2) . 2_554
F5 Mo1 O17 K4 -147.3(5) . 2_554
F5 K3 F9 Mo1 66.27(18) 2 .
F5 K3 F9 Mo2 -120.81(15) 2 .
F5 K3 F9 K1 -27.06(16) 2 .
F5 K3 F9 K2 150.73(12) 2 .
F5 K3 F11 Mo2 150.43(19) 2 .
F5 K3 F11 K1 52.84(14) 2 .
F5 K3 F11 K4 -56.8(2) 2 .
F5 K3 F12 Mo2 22.4(5) 2 .
F5 K3 F12 K2 136.8(3) 2 .
F5 K3 F12 K6 -120.0(3) 2 .
F6 Mo2 F9 Mo1 -85.8(11) . .
F6 Mo2 F9 K1 40.44(16) . .
F6 Mo2 F9 K2 -141.06(16) . .
F6 Mo2 F9 K3 131.47(18) . .
F6 Mo2 F9 K4 -46.22(15) . 2_564
F6 Mo2 F11 K1 -30.14(18) . .
F6 Mo2 F11 K3 -121.5(2) . .
F6 Mo2 F11 K4 90.5(3) . .
F6 Mo2 F12 K2 -46.8(7) . .
F6 Mo2 F12 K3 51.4(6) . .
F6 Mo2 F12 K6 177.6(4) . .
F6 Mo2 O16 K3 19.4(8) . 1_565
F6 K1 F3 Mo4 -73.1(3) . .
F6 K1 F3 K2 38.60(13) . 2_565
F6 K1 F3 K6 134.4(2) . 2_565
F6 K1 F4 Mo1 -94.18(18) . .
F6 K1 F4 K4 13.64(13) . 2_564
F6 K1 F4 K5 138.88(16) . .
F6 K1 F7 Mo1 27.4(4) . 2
F6 K1 F7 K2 137.0(2) . 2
F6 K1 F7 K3 -122.0(2) . 2
F6 K1 F8 Mo2 -138.7(3) . 2_565
F6 K1 F8 K2 -39.95(12) . 2_565
F6 K1 F8 K4 73.2(2) . .
F6 K1 F9 Mo1 137.7(2) . .
F6 K1 F9 Mo2 -32.88(15) . .
F6 K1 F9 K3 -129.39(17) . .
F6 K1 F9 K4 50.60(14) . 2_564
F6 K1 F11 Mo2 25.19(15) . .
F6 K1 F11 K3 129.33(17) . .
F6 K1 F11 K4 -111.4(2) . .
F6 K2 F5 Mo1 172.7(2) 2_564 .
F6 K2 F5 K3 -76.07(16) 2_564 2_554
F6 K2 F5 K4 66.88(16) 2_564 2_564
F6 K2 F9 Mo1 -92.17(16) 2_564 .
F6 K2 F9 Mo2 78.16(17) 2_564 .
F6 K2 F9 K3 174.67(13) 2_564 .
F6 K2 F9 K4 -5.40(15) 2_564 2_564
F6 K2 F10 Mo1 -70.5(3) 2_564 2_554
F6 K2 F10 K1 179.40(16) 2_564 2_554
F6 K2 F10 K3 83.06(18) 2_564 2_554
F6 K2 F12 Mo2 -50.7(3) 2_564 .
F6 K2 F12 K3 -149.74(14) 2_564 .
F6 K2 F12 K6 99.00(18) 2_564 .
F6 K4 F8 Mo2 -16.51(17) 2_565 2_565
F6 K4 F8 K1 138.4(3) 2_565 .
F6 K4 F8 K2 -123.66(19) 2_565 2_565
F6 K4 F11 Mo2 -124.2(3) 2_565 .
F6 K4 F11 K1 -7.7(2) 2_565 .
F6 K4 F11 K3 91.4(2) 2_565 .
F7 Mo1 F4 K1 45.1(6) 2_554 .
F7 Mo1 F4 K4 -56.6(6) 2_554 2_564
F7 Mo1 F4 K5 162.5(5) 2_554 .
F7 Mo1 F5 K2 23.54(19) 2_554 .
F7 Mo1 F5 K3 -87.95(19) 2_554 2_554
F7 Mo1 F5 K4 135.81(17) 2_554 2_564
F7 Mo1 F9 Mo2 -98.2(11) 2_554 .
F7 Mo1 F9 K1 135.50(17) 2_554 .
F7 Mo1 F9 K2 -42.62(15) 2_554 .
F7 Mo1 F9 K3 44.73(16) 2_554 .
F7 Mo1 F9 K4 -137.57(16) 2_554 2_564
F7 Mo1 O17 K3 80.9(2) 2_554 2_554
F7 Mo1 O17 K4 -57.3(6) 2_554 2_554
F7 K1 F3 Mo4 140.5(2) . .
F7 K1 F3 K2 -107.84(16) . 2_565
F7 K1 F3 K6 -12.0(3) . 2_565
F7 K1 F4 Mo1 55.8(2) . .
F7 K1 F4 K4 163.62(14) . 2_564
F7 K1 F4 K5 -71.1(2) . .
F7 K1 F6 Mo2 -45.1(3) . .
F7 K1 F6 K2 92.0(2) . 2_565
F7 K1 F6 K4 -151.4(2) . 2_564
F7 K1 F8 Mo2 66.7(3) . 2_565
F7 K1 F8 K2 165.47(15) . 2_565
F7 K1 F8 K4 -81.4(2) . .
F7 K1 F9 Mo1 -83.22(17) . .
F7 K1 F9 Mo2 106.25(16) . .
F7 K1 F9 K3 9.74(16) . .
F7 K1 F9 K4 -170.28(12) . 2_564
F7 K1 F11 Mo2 -166.34(18) . .
F7 K1 F11 K3 -62.20(13) . .
F7 K1 F11 K4 57.11(17) . .
F7 K2 F5 Mo1 -19.72(16) 2_554 .
F7 K2 F5 K3 91.49(18) 2_554 2_554
F7 K2 F5 K4 -125.55(19) 2_554 2_564
F7 K2 F9 Mo1 36.78(15) 2_554 .
F7 K2 F9 Mo2 -152.9(2) 2_554 .
F7 K2 F9 K3 -56.38(15) 2_554 .
F7 K2 F9 K4 123.55(17) 2_554 2_564
F7 K2 F10 Mo1 149.2(3) 2_554 2_554
F7 K2 F10 K1 39.04(12) 2_554 2_554
F7 K2 F10 K3 -57.31(17) 2_554 2_554
F7 K2 F12 Mo2 83.2(2) 2_554 .
F7 K2 F12 K3 -15.86(12) 2_554 .
F7 K2 F12 K6 -127.12(18) 2_554 .
F7 K3 F9 Mo1 -34.75(13) 2_554 .
F7 K3 F9 Mo2 138.2(2) 2_554 .
F7 K3 F9 K1 -128.09(16) 2_554 .
F7 K3 F9 K2 49.70(12) 2_554 .
F7 K3 F11 Mo2 29.2(2) 2_554 .
F7 K3 F11 K1 -68.34(14) 2_554 .
F7 K3 F11 K4 -178.02(17) 2_554 .
F7 K3 F12 Mo2 -98.55(18) 2_554 .
F7 K3 F12 K2 15.85(12) 2_554 .
F7 K3 F12 K6 118.98(18) 2_554 .
F8 Mo2 F6 K1 -124.8(2) 2_564 .
F8 Mo2 F6 K2 128.7(3) 2_564 2_565
F8 Mo2 F6 K4 -19.82(19) 2_564 2_564
F8 Mo2 F9 Mo1 4.4(11) 2_564 .
F8 Mo2 F9 K1 130.66(18) 2_564 .
F8 Mo2 F9 K2 -50.84(16) 2_564 .
F8 Mo2 F9 K3 -138.32(19) 2_564 .
F8 Mo2 F9 K4 43.99(16) 2_564 2_564
F8 Mo2 F11 K1 51.9(6) 2_564 .
F8 Mo2 F11 K3 -39.5(6) 2_564 .
F8 Mo2 F11 K4 172.6(4) 2_564 .
F8 Mo2 F12 K2 27.8(2) 2_564 .
F8 Mo2 F12 K3 126.00(18) 2_564 .
F8 Mo2 F12 K6 -107.9(4) 2_564 .
F8 Mo2 O16 K3 -70.5(8) 2_564 1_565
F8 K1 F3 Mo4 -152.2(3) . .
F8 K1 F3 K2 -40.54(14) . 2_565
F8 K1 F3 K6 55.30(19) . 2_565
F8 K1 F4 Mo1 -98.1(4) . .
F8 K1 F4 K4 9.8(4) . 2_564
F8 K1 F4 K5 135.0(3) . .
F8 K1 F6 Mo2 -89.2(2) . .
F8 K1 F6 K2 47.82(15) . 2_565
F8 K1 F6 K4 164.44(17) . 2_564
F8 K1 F7 Mo1 72.3(3) . 2
F8 K1 F7 K2 -178.22(16) . 2
F8 K1 F7 K3 -77.2(2) . 2
F8 K1 F9 Mo1 -166.61(16) . .
F8 K1 F9 Mo2 22.9(2) . .
F8 K1 F9 K3 -73.65(16) . .
F8 K1 F9 K4 106.34(14) . 2_564
F8 K1 F11 Mo2 120.7(2) . .
F8 K1 F11 K3 -135.13(17) . .
F8 K1 F11 K4 -15.83(16) . .
F8 K4 F11 Mo2 -101.8(3) . .
F8 K4 F11 K1 14.76(15) . .
F8 K4 F11 K3 113.8(2) . .
F9 Mo1 F4 K1 46.82(15) . .
F9 Mo1 F4 K4 -54.83(17) . 2_564
F9 Mo1 F4 K5 164.2(2) . .
F9 Mo1 F5 K2 -57.71(17) . .
F9 Mo1 F5 K3 -169.20(19) . 2_554
F9 Mo1 F5 K4 54.56(16) . 2_564
F9 Mo2 F6 K1 -45.26(17) . .
F9 Mo2 F6 K2 -151.8(3) . 2_565
F9 Mo2 F6 K4 59.66(17) . 2_564
F9 Mo2 F11 K1 49.14(15) . .
F9 Mo2 F11 K3 -42.22(17) . .
F9 Mo2 F11 K4 169.8(3) . .
F9 Mo2 F12 K2 -52.1(2) . .
F9 Mo2 F12 K3 46.10(15) . .
F9 Mo2 F12 K6 172.2(4) . .
F9 K3 F11 Mo2 38.05(16) . .
F9 K3 F11 K1 -59.54(13) . .
F9 K3 F11 K4 -169.2(3) . .
F9 K3 F12 Mo2 -42.82(15) . .
F9 K3 F12 K2 71.58(15) . .
F9 K3 F12 K6 174.7(2) . .
F10 Mo1 F4 K1 -30.53(17) 2 .
F10 Mo1 F4 K4 -132.17(19) 2 2_564
F10 Mo1 F4 K5 86.9(2) 2 .
F10 Mo1 F5 K2 -60.2(6) 2 .
F10 Mo1 F5 K3 -171.7(5) 2 2_554
F10 Mo1 F5 K4 52.0(6) 2 2_564
F10 Mo1 F9 Mo2 170.5(11) 2 .
F10 Mo1 F9 K1 44.23(15) 2 .
F10 Mo1 F9 K2 -133.89(16) 2 .
F10 Mo1 F9 K3 -46.55(15) 2 .
F10 Mo1 F9 K4 131.15(16) 2 2_564
F10 Mo1 O17 K3 171.65(17) 2 2_554
F10 Mo1 O17 K4 33.4(6) 2 2_554
F10 K1 F3 Mo4 24.4(4) 2 .
F10 K1 F3 K2 136.07(18) 2 2_565
F10 K1 F3 K6 -128.1(2) 2 2_565
F10 K1 F4 Mo1 25.38(15) 2 .
F10 K1 F4 K4 133.20(18) 2 2_564
F10 K1 F4 K5 -101.56(19) 2 .
F10 K1 F6 Mo2 44.0(2) 2 .
F10 K1 F6 K2 -179.03(13) 2 2_565
F10 K1 F6 K4 -62.40(17) 2 2_564
F10 K1 F7 Mo1 -71.8(3) 2 2
F10 K1 F7 K2 37.71(12) 2 2
F10 K1 F7 K3 138.7(2) 2 2
F10 K1 F8 Mo2 119.7(3) 2 2_565
F10 K1 F8 K2 -141.57(16) 2 2_565
F10 K1 F8 K4 -28.4(3) 2 .
F10 K1 F9 Mo1 -36.60(14) 2 .
F10 K1 F9 Mo2 152.9(2) 2 .
F10 K1 F9 K3 56.36(14) 2 .
F10 K1 F9 K4 -123.65(16) 2 2_564
F10 K1 F11 Mo2 -90.26(18) 2 .
F10 K1 F11 K3 13.88(12) 2 .
F10 K1 F11 K4 133.18(16) 2 .
F10 K2 F5 Mo1 -110.2(2) . .
F10 K2 F5 K3 0.96(14) . 2_554
F10 K2 F5 K4 143.91(18) . 2_564
F10 K2 F9 Mo1 -11.84(18) . .
F10 K2 F9 Mo2 158.49(14) . .
F10 K2 F9 K3 -105.00(14) . .
F10 K2 F9 K4 74.93(14) . 2_564
F10 K2 F12 Mo2 72.4(5) . .
F10 K2 F12 K3 -26.7(5) . .
F10 K2 F12 K6 -137.9(4) . .
F10 K3 F9 Mo1 37.88(14) 2 .
F10 K3 F9 Mo2 -149.2(2) 2 .
F10 K3 F9 K1 -55.46(13) 2 .
F10 K3 F9 K2 122.33(15) 2 .
F10 K3 F11 Mo2 83.7(2) 2 .
F10 K3 F11 K1 -13.86(12) 2 .
F10 K3 F11 K4 -123.54(19) 2 .
F10 K3 F12 Mo2 -47.7(2) 2 .
F10 K3 F12 K2 66.67(15) 2 .
F10 K3 F12 K6 169.80(16) 2 .
F11 Mo2 F6 K1 34.0(2) . .
F11 Mo2 F6 K2 -72.5(3) . 2_565
F11 Mo2 F6 K4 138.97(19) . 2_564
F11 Mo2 F9 Mo1 -176.6(11) . .
F11 Mo2 F9 K1 -50.37(17) . .
F11 Mo2 F9 K2 128.13(17) . .
F11 Mo2 F9 K3 40.66(17) . .
F11 Mo2 F9 K4 -137.03(17) . 2_564
F11 Mo2 F12 K2 -131.4(2) . .
F11 Mo2 F12 K3 -33.14(18) . .
F11 Mo2 F12 K6 93.0(4) . .
F11 Mo2 O16 K3 110.5(8) . 1_565
F11 K3 F9 Mo1 155.4(2) . .
F11 K3 F9 Mo2 -31.69(14) . .
F11 K3 F9 K1 62.06(14) . .
F11 K3 F9 K2 -120.15(16) . .
F11 K3 F12 Mo2 26.93(15) . .
F11 K3 F12 K2 141.32(19) . .
F11 K3 F12 K6 -115.5(2) . .
F11 K4 F8 Mo2 -174.0(2) . 2_565
F11 K4 F8 K1 -19.07(19) . .
F11 K4 F8 K2 78.88(16) . 2_565
F12 Mo2 F6 K1 -50.6(6) . .
F12 Mo2 F6 K2 -157.1(5) . 2_565
F12 Mo2 F6 K4 54.3(6) . 2_564
F12 Mo2 F9 Mo1 92.2(11) . .
F12 Mo2 F9 K1 -141.5(2) . .
F12 Mo2 F9 K2 36.96(16) . .
F12 Mo2 F9 K3 -50.52(18) . .
F12 Mo2 F9 K4 131.79(18) . 2_564
F12 Mo2 F11 K1 128.53(18) . .
F12 Mo2 F11 K3 37.2(2) . .
F12 Mo2 F11 K4 -110.8(3) . .
F12 Mo2 O16 K3 -158.1(8) . 1_565
F12 K2 F5 Mo1 56.0(2) . .
F12 K2 F5 K3 167.19(16) . 2_554
F12 K2 F5 K4 -49.86(18) . 2_564
F12 K2 F9 Mo1 157.4(2) . .
F12 K2 F9 Mo2 -32.23(15) . .
F12 K2 F9 K3 64.28(16) . .
F12 K2 F9 K4 -115.79(18) . 2_564
F12 K2 F10 Mo1 160.1(3) . 2_554
F12 K2 F10 K1 50.0(5) . 2_554
F12 K2 F10 K3 -46.3(5) . 2_554
F12 K6 F12 Mo2 -117.1(5) 3 .
F12 K6 F12 K2 103.6(6) 3 .
F12 K6 F12 K3 4.3(7) 3 .
F13 Mo3 F2 K1 -159.3(6) . 3_655
F13 Mo3 F2 K1 -67.1(3) 3_655 3_655
F13 Mo3 F2 K2 30.3(2) 3_655 4
F13 Mo3 F2 K2 -61.9(7) . 4
F13 Mo3 F2 K5 145.3(2) 3_655 .
F13 Mo3 F2 K5 53.1(7) . .
F13 Mo3 F13 K2 -128.51(17) 3_655 2
F13 Mo3 F13 K3 94.0(5) 3_655 2
F13 Mo3 F13 K6 -41.0(3) 3_655 2
F13 Mo3 O18 K6 131.9(2) 3_655 2_565
F13 Mo3 O18 K6 -131.9(2) . 2_565
F13 K3 F9 Mo1 -95.31(17) 2_554 .
F13 K3 F9 Mo2 77.60(17) 2_554 .
F13 K3 F9 K1 171.35(15) 2_554 .
F13 K3 F9 K2 -10.85(14) 2_554 .
F13 K3 F11 Mo2 -42.6(3) 2_554 .
F13 K3 F11 K1 -140.15(15) 2_554 .
F13 K3 F11 K4 110.2(2) 2_554 .
F13 K3 F12 Mo2 -170.2(3) 2_554 .
F13 K3 F12 K2 -55.84(18) 2_554 .
F13 K3 F12 K6 47.3(2) 2_554 .
F13 K6 F12 Mo2 -153.8(3) 4_454 .
F13 K6 F12 K2 66.9(2) 4_454 .
F13 K6 F12 K3 -32.4(2) 4_454 .
F14 Mo3 F2 K1 -149.2(3) 1_545 3_655
F14 Mo3 F2 K2 -51.80(16) 1_545 4
F14 Mo3 F2 K5 63.18(19) 1_545 .
F14 Mo3 F13 K2 -47.56(19) 1_545 2
F14 Mo3 F13 K3 175.0(5) 1_545 2
F14 Mo3 F13 K6 39.94(17) 1_545 2
F14 Mo4 F1 K2 -52.22(17) . 2_565
F14 Mo4 F1 K4 -164.4(2) . 2_564
F14 Mo4 F1 K5 58.36(18) . 1_565
F14 Mo4 F3 K1 159.2(3) . .
F14 Mo4 F3 K2 53.53(17) . 2_565
F14 Mo4 F3 K6 -43.39(15) . 2_565
F14 K6 F12 Mo2 154.2(4) 2_564 .
F14 K6 F12 K2 14.87(19) 2_564 .
F14 K6 F12 K3 -84.41(18) 2_564 .
O1 Mo4 F1 K2 -134.53(10) 3_655 2_565
O1 Mo4 F1 K4 113.28(16) 3_655 2_564
O1 Mo4 F1 K5 -23.9(3) 3_655 1_565
O1 Mo4 F3 K1 156.3(5) 3_655 .
O1 Mo4 F3 K2 50.6(6) 3_655 2_565
O1 Mo4 F3 K6 -46.3(6) 3_655 2_565
O1 Mo4 F14 Mo3 45.09(14) 3_655 1_565
O1 Mo4 F14 K2 -45.71(17) 3_655 4_565
O1 Mo4 F14 K2 135.90(19) 3_655 2_565
O1 Mo4 F14 K5 45.09(14) 3_655 1_565
O1 Mo4 F14 K6 -134.91(14) 3_655 2_565
O1 Mo4 O19 K4 -101.90(18) 3_655 2_564
O1 Mo4 O19 K4 11.1(2) 3_655 4_564
O1 Mo4 O19 K5 134.60(14) 3_655 .
O1 K2 F5 Mo1 -150.06(18) 2_564 .
O1 K2 F5 K3 -38.9(3) 2_564 2_554
O1 K2 F5 K4 104.1(2) 2_564 2_564
O1 K2 F9 Mo1 -170.1(5) 2_564 .
O1 K2 F9 Mo2 0.2(6) 2_564 .
O1 K2 F9 K3 96.8(5) 2_564 .
O1 K2 F9 K4 -83.3(5) 2_564 2_564
O1 K2 F10 Mo1 0.1(3) 2_564 2_554
O1 K2 F10 K1 -110.00(14) 2_564 2_554
O1 K2 F10 K3 153.66(19) 2_564 2_554
O1 K2 F12 Mo2 -130.2(2) 2_564 .
O1 K2 F12 K3 130.78(14) 2_564 .
O1 K2 F12 K6 19.5(2) 2_564 .
O1 K4 F8 Mo2 -53.7(2) 2_565 2_565
O1 K4 F8 K1 101.2(2) 2_565 .
O1 K4 F8 K2 -160.81(13) 2_565 2_565
O1 K4 F11 Mo2 151.0(2) 2_565 .
O1 K4 F11 K1 -92.4(2) 2_565 .
O1 K4 F11 K3 6.6(3) 2_565 .
O1 K5 F2 Mo3 -99.8(2) 3_645 .
O1 K5 F2 Mo3 -50.8(2) 1_545 .
O1 K5 F2 K1 107.8(2) 3_645 3_655
O1 K5 F2 K1 156.77(19) 1_545 3_655
O1 K5 F2 K2 59.32(17) 1_545 4
O1 K5 F2 K2 10.32(13) 3_645 4
O1 K5 F4 Mo1 -27.1(4) 3_645 .
O1 K5 F4 Mo1 -30.3(2) 1_545 .
O1 K5 F4 K1 87.6(3) 3_645 .
O1 K5 F4 K1 84.42(16) 1_545 .
O1 K5 F4 K4 -162.3(2) 3_645 2_564
O1 K5 F4 K4 -165.54(18) 1_545 2_564
O1 K5 O19 Mo4 -63.7(3) 3_645 .
O1 K5 O19 Mo4 63.7(3) 1_545 .
O1 K5 O19 K4 58.9(4) 3_645 4_564
O1 K5 O19 K4 173.8(2) 3_645 2_564
O1 K5 O19 K4 -173.8(2) 1_545 4_564
O1 K5 O19 K4 -58.9(4) 1_545 2_564
O2 Mo3 F2 K1 132.2(2) 3_655 3_655
O2 Mo3 F2 K2 -130.43(12) 3_655 4
O2 Mo3 F2 K5 -15.4(3) 3_655 .
O2 Mo3 F13 K2 30.7(2) 3_655 2
O2 Mo3 F13 K3 -106.8(5) 3_655 2
O2 Mo3 F13 K6 118.2(2) 3_655 2
O2 Mo3 O18 K6 -43.39(15) 3_655 2_565
O2 K1 F3 Mo4 72.0(3) 3_655 .
O2 K1 F3 K2 -176.29(15) 3_655 2_565
O2 K1 F3 K6 -80.45(19) 3_655 2_565
O2 K1 F4 Mo1 115.2(2) 3_655 .
O2 K1 F4 K4 -136.99(18) 3_655 2_564
O2 K1 F4 K5 -11.75(15) 3_655 .
O2 K1 F6 Mo2 131.7(2) 3_655 .
O2 K1 F6 K2 -91.3(2) 3_655 2_565
O2 K1 F6 K4 25.3(3) 3_655 2_564
O2 K1 F7 Mo1 -150.2(3) 3_655 2
O2 K1 F7 K2 -40.70(14) 3_655 2
O2 K1 F7 K3 60.3(2) 3_655 2
O2 K1 F8 Mo2 2.5(4) 3_655 2_565
O2 K1 F8 K2 101.2(2) 3_655 2_565
O2 K1 F8 K4 -145.6(2) 3_655 .
O2 K1 F9 Mo1 9.8(2) 3_655 .
O2 K1 F9 Mo2 -160.72(16) 3_655 .
O2 K1 F9 K3 102.77(16) 3_655 .
O2 K1 F9 K4 -77.24(16) 3_655 2_564
O2 K1 F11 Mo2 -99.6(4) 3_655 .
O2 K1 F11 K3 4.6(5) 3_655 .
O2 K1 F11 K4 123.9(4) 3_655 .
O2 K5 F2 Mo3 13.0(2) 3_655 .
O2 K5 F2 K1 -139.40(14) 3_655 3_655
O2 K5 F2 K2 123.14(11) 3_655 4
O2 K5 F4 Mo1 -103.4(2) 3_655 .
O2 K5 F4 K1 11.32(14) 3_655 .
O2 K5 F4 K4 121.4(2) 3_655 2_564
O2 K5 O19 Mo4 30.10(10) 3_655 .
O2 K5 O19 K4 152.65(19) 3_655 4_564
O2 K5 O19 K4 -92.45(17) 3_655 2_564
O3 Mo4 F1 K2 -55.1(6) 3_655 2_565
O3 Mo4 F1 K4 -167.3(5) 3_655 2_564
O3 Mo4 F1 K5 55.5(6) 3_655 1_565
O3 Mo4 F3 K1 -121.8(2) 3_655 .
O3 Mo4 F3 K2 132.48(10) 3_655 2_565
O3 Mo4 F3 K6 35.6(2) 3_655 2_565
O3 Mo4 F14 Mo3 133.97(13) 3_655 1_565
O3 Mo4 F14 K2 -135.22(19) 3_655 2_565
O3 Mo4 F14 K2 43.17(16) 3_655 4_565
O3 Mo4 F14 K5 133.97(13) 3_655 1_565
O3 Mo4 F14 K6 -46.03(13) 3_655 2_565
O3 Mo4 O19 K4 -77.8(2) 3_655 4_564
O3 Mo4 O19 K4 169.17(17) 3_655 2_564
O3 Mo4 O19 K5 45.68(13) 3_655 .
O3 K2 F5 Mo1 120.8(2) 2_564 .
O3 K2 F5 K3 -127.95(19) 2_564 2_554
O3 K2 F5 K4 15.0(3) 2_564 2_564
O3 K2 F9 Mo1 -173.32(13) 2_564 .
O3 K2 F9 Mo2 -3.00(17) 2_564 .
O3 K2 F9 K3 93.52(13) 2_564 .
O3 K2 F9 K4 -86.56(13) 2_564 2_564
O3 K2 F10 Mo1 -18.1(4) 2_564 2_554
O3 K2 F10 K1 -128.18(15) 2_564 2_554
O3 K2 F10 K3 135.48(17) 2_564 2_554
O3 K2 F12 Mo2 -109.1(3) 2_564 .
O3 K2 F12 K3 151.87(15) 2_564 .
O3 K2 F12 K6 40.61(15) 2_564 .
O3 K6 F12 Mo2 108.1(3) 4_464 .
O3 K6 F12 Mo2 100.2(4) 2_564 .
O3 K6 F12 K2 -31.3(2) 4_464 .
O3 K6 F12 K2 -39.15(14) 2_564 .
O3 K6 F12 K3 -138.43(18) 2_564 .
O3 K6 F12 K3 -130.53(16) 4_464 .
O4 K4 F8 Mo2 53.8(2) 2_565 2_565
O4 K4 F8 K1 -151.4(2) 2_565 .
O4 K4 F8 K2 -53.40(17) 2_565 2_565
O4 K4 F11 Mo2 -18.5(4) 2_565 .
O4 K4 F11 K1 98.0(2) 2_565 .
O4 K4 F11 K3 -162.89(16) 2_565 .
O4 K5 F2 Mo3 165.8(2) 3_655 .
O4 K5 F2 K1 13.43(17) 3_655 3_655
O4 K5 F2 K2 -84.02(16) 3_655 4
O4 K5 F4 Mo1 144.82(14) 3_655 .
O4 K5 F4 K1 -100.5(2) 3_655 .
O4 K5 F4 K4 9.6(4) 3_655 2_564
O4 K5 O19 Mo4 -99.41(12) 3_655 .
O4 K5 O19 K4 138.0(2) 3_655 2_564
O4 K5 O19 K4 23.14(14) 3_655 4_564
O5 K3 F9 Mo1 66.27(18) 2 .
O5 K3 F9 Mo2 -120.81(15) 2 .
O5 K3 F9 K1 -27.06(16) 2 .
O5 K3 F9 K2 150.73(12) 2 .
O5 K3 F11 Mo2 150.43(19) 2 .
O5 K3 F11 K1 52.84(14) 2 .
O5 K3 F11 K4 -56.8(2) 2 .
O5 K3 F12 Mo2 22.4(5) 2 .
O5 K3 F12 K2 136.8(3) 2 .
O5 K3 F12 K6 -120.0(3) 2 .
O5 K4 F8 Mo2 99.5(2) 2_565 2_565
O5 K4 F8 K1 -105.7(2) 2_565 .
O5 K4 F8 K2 -7.70(13) 2_565 2_565
O5 K4 F11 Mo2 -27.7(3) 2_565 .
O5 K4 F11 K1 88.92(15) 2_565 .
O5 K4 F11 K3 -172.0(2) 2_565 .
O6 K2 F5 Mo1 172.7(2) 2_564 .
O6 K2 F5 K3 -76.07(16) 2_564 2_554
O6 K2 F5 K4 66.88(16) 2_564 2_564
O6 K2 F9 Mo1 -92.17(16) 2_564 .
O6 K2 F9 Mo2 78.16(17) 2_564 .
O6 K2 F9 K3 174.67(13) 2_564 .
O6 K2 F9 K4 -5.40(15) 2_564 2_564
O6 K2 F10 Mo1 -70.5(3) 2_564 2_554
O6 K2 F10 K1 179.40(16) 2_564 2_554
O6 K2 F10 K3 83.06(18) 2_564 2_554
O6 K2 F12 Mo2 -50.7(3) 2_564 .
O6 K2 F12 K3 -149.74(14) 2_564 .
O6 K2 F12 K6 99.00(18) 2_564 .
O6 K4 F8 Mo2 -16.51(17) 2_565 2_565
O6 K4 F8 K1 138.4(3) 2_565 .
O6 K4 F8 K2 -123.66(19) 2_565 2_565
O6 K4 F11 Mo2 -124.2(3) 2_565 .
O6 K4 F11 K1 -7.7(2) 2_565 .
O6 K4 F11 K3 91.4(2) 2_565 .
O7 Mo1 F4 K1 45.1(6) 2_554 .
O7 Mo1 F4 K4 -56.6(6) 2_554 2_564
O7 Mo1 F4 K5 162.5(5) 2_554 .
O7 Mo1 F5 K2 23.54(19) 2_554 .
O7 Mo1 F5 K3 -87.95(19) 2_554 2_554
O7 Mo1 F5 K4 135.81(17) 2_554 2_564
O7 Mo1 F9 Mo2 -98.2(11) 2_554 .
O7 Mo1 F9 K1 135.50(17) 2_554 .
O7 Mo1 F9 K2 -42.62(15) 2_554 .
O7 Mo1 F9 K3 44.73(16) 2_554 .
O7 Mo1 F9 K4 -137.57(16) 2_554 2_564
O7 Mo1 O17 K3 80.9(2) 2_554 2_554
O7 Mo1 O17 K4 -57.3(6) 2_554 2_554
O7 K2 F5 Mo1 -19.72(16) 2_554 .
O7 K2 F5 K3 91.49(18) 2_554 2_554
O7 K2 F5 K4 -125.55(19) 2_554 2_564
O7 K2 F9 Mo1 36.78(15) 2_554 .
O7 K2 F9 Mo2 -152.9(2) 2_554 .
O7 K2 F9 K3 -56.38(15) 2_554 .
O7 K2 F9 K4 123.55(17) 2_554 2_564
O7 K2 F10 Mo1 149.2(3) 2_554 2_554
O7 K2 F10 K1 39.04(12) 2_554 2_554
O7 K2 F10 K3 -57.31(17) 2_554 2_554
O7 K2 F12 Mo2 83.2(2) 2_554 .
O7 K2 F12 K3 -15.86(12) 2_554 .
O7 K2 F12 K6 -127.12(18) 2_554 .
O7 K3 F9 Mo1 -34.75(13) 2_554 .
O7 K3 F9 Mo2 138.2(2) 2_554 .
O7 K3 F9 K1 -128.09(16) 2_554 .
O7 K3 F9 K2 49.70(12) 2_554 .
O7 K3 F11 Mo2 29.2(2) 2_554 .
O7 K3 F11 K1 -68.34(14) 2_554 .
O7 K3 F11 K4 -178.02(17) 2_554 .
O7 K3 F12 Mo2 -98.55(18) 2_554 .
O7 K3 F12 K2 15.85(12) 2_554 .
O7 K3 F12 K6 118.98(18) 2_554 .
O8 Mo2 F6 K1 -124.8(2) 2_564 .
O8 Mo2 F6 K2 128.7(3) 2_564 2_565
O8 Mo2 F6 K4 -19.82(19) 2_564 2_564
O8 Mo2 F9 Mo1 4.4(11) 2_564 .
O8 Mo2 F9 K1 130.66(18) 2_564 .
O8 Mo2 F9 K2 -50.84(16) 2_564 .
O8 Mo2 F9 K3 -138.32(19) 2_564 .
O8 Mo2 F9 K4 43.99(16) 2_564 2_564
O8 Mo2 F11 K1 51.9(6) 2_564 .
O8 Mo2 F11 K3 -39.5(6) 2_564 .
O8 Mo2 F11 K4 172.6(4) 2_564 .
O8 Mo2 F12 K2 27.8(2) 2_564 .
O8 Mo2 F12 K3 126.00(18) 2_564 .
O8 Mo2 F12 K6 -107.9(4) 2_564 .
O8 Mo2 O16 K3 -70.5(8) 2_564 1_565
O10 Mo1 F4 K1 -30.53(17) 2 .
O10 Mo1 F4 K4 -132.17(19) 2 2_564
O10 Mo1 F4 K5 86.9(2) 2 .
O10 Mo1 F5 K2 -60.2(6) 2 .
O10 Mo1 F5 K3 -171.7(5) 2 2_554
O10 Mo1 F5 K4 52.0(6) 2 2_564
O10 Mo1 F9 Mo2 170.5(11) 2 .
O10 Mo1 F9 K1 44.23(15) 2 .
O10 Mo1 F9 K2 -133.89(16) 2 .
O10 Mo1 F9 K3 -46.55(15) 2 .
O10 Mo1 F9 K4 131.15(16) 2 2_564
O10 Mo1 O17 K3 171.65(17) 2 2_554
O10 Mo1 O17 K4 33.4(6) 2 2_554
O10 K1 F3 Mo4 24.4(4) 2 .
O10 K1 F3 K2 136.07(18) 2 2_565
O10 K1 F3 K6 -128.1(2) 2 2_565
O10 K1 F4 Mo1 25.38(15) 2 .
O10 K1 F4 K4 133.20(18) 2 2_564
O10 K1 F4 K5 -101.56(19) 2 .
O10 K1 F6 Mo2 44.0(2) 2 .
O10 K1 F6 K2 -179.03(13) 2 2_565
O10 K1 F6 K4 -62.40(17) 2 2_564
O10 K1 F7 Mo1 -71.8(3) 2 2
O10 K1 F7 K2 37.71(12) 2 2
O10 K1 F7 K3 138.7(2) 2 2
O10 K1 F8 Mo2 119.7(3) 2 2_565
O10 K1 F8 K2 -141.57(16) 2 2_565
O10 K1 F8 K4 -28.4(3) 2 .
O10 K1 F9 Mo1 -36.60(14) 2 .
O10 K1 F9 Mo2 152.9(2) 2 .
O10 K1 F9 K3 56.36(14) 2 .
O10 K1 F9 K4 -123.65(16) 2 2_564
O10 K1 F11 Mo2 -90.26(18) 2 .
O10 K1 F11 K3 13.88(12) 2 .
O10 K1 F11 K4 133.18(16) 2 .
O10 K3 F9 Mo1 37.88(14) 2 .
O10 K3 F9 Mo2 -149.2(2) 2 .
O10 K3 F9 K1 -55.46(13) 2 .
O10 K3 F9 K2 122.33(15) 2 .
O10 K3 F11 Mo2 83.7(2) 2 .
O10 K3 F11 K1 -13.86(12) 2 .
O10 K3 F11 K4 -123.54(19) 2 .
O10 K3 F12 Mo2 -47.7(2) 2 .
O10 K3 F12 K2 66.67(15) 2 .
O10 K3 F12 K6 169.80(16) 2 .
O12 K6 F12 Mo2 -117.1(5) 3 .
O12 K6 F12 K2 103.6(6) 3 .
O12 K6 F12 K3 4.3(7) 3 .
O13 Mo3 F2 K1 -67.1(3) 3_655 3_655
O13 Mo3 F2 K2 30.3(2) 3_655 4
O13 Mo3 F2 K5 145.3(2) 3_655 .
O13 Mo3 F13 K2 -128.51(17) 3_655 2
O13 Mo3 F13 K3 94.0(5) 3_655 2
O13 Mo3 F13 K6 -41.0(3) 3_655 2
O13 Mo3 O18 K6 131.9(2) 3_655 2_565
O13 K3 F9 Mo1 -95.31(17) 2_554 .
O13 K3 F9 Mo2 77.60(17) 2_554 .
O13 K3 F9 K1 171.35(15) 2_554 .
O13 K3 F9 K2 -10.85(14) 2_554 .
O13 K3 F11 Mo2 -42.6(3) 2_554 .
O13 K3 F11 K1 -140.15(15) 2_554 .
O13 K3 F11 K4 110.2(2) 2_554 .
O13 K3 F12 Mo2 -170.2(3) 2_554 .
O13 K3 F12 K2 -55.84(18) 2_554 .
O13 K3 F12 K6 47.3(2) 2_554 .
O13 K6 F12 Mo2 -153.8(3) 4_454 .
O13 K6 F12 K2 66.9(2) 4_454 .
O13 K6 F12 K3 -32.4(2) 4_454 .
O16 Mo2 F6 K1 136.2(2) . .
O16 Mo2 F6 K2 29.7(4) . 2_565
O16 Mo2 F6 K4 -118.9(2) . 2_564
O16 Mo2 F11 K1 -130.8(2) . .
O16 Mo2 F11 K3 137.8(2) . .
O16 Mo2 F11 K4 -10.2(3) . .
O16 Mo2 F12 K2 126.4(3) . .
O16 Mo2 F12 K3 -135.4(2) . .
O16 Mo2 F12 K6 -9.3(4) . .
O16 K3 F9 Mo1 -3.9(2) 1_545 .
O16 K3 F9 Mo2 168.99(16) 1_545 .
O16 K3 F9 K1 -97.26(16) 1_545 .
O16 K3 F9 K2 80.53(17) 1_545 .
O16 K3 F11 Mo2 107.3(5) 1_545 .
O16 K3 F11 K1 9.7(5) 1_545 .
O16 K3 F11 K4 -100.0(5) 1_545 .
O16 K3 F12 Mo2 -131.9(2) 1_545 .
O16 K3 F12 K2 -17.5(3) 1_545 .
O16 K3 F12 K6 85.6(3) 1_545 .
O17 Mo1 F4 K1 -130.2(2) . .
O17 Mo1 F4 K4 128.1(2) . 2_564
O17 Mo1 F4 K5 -12.8(3) . .
O17 Mo1 F5 K2 121.7(2) . .
O17 Mo1 F5 K3 10.2(3) . 2_554
O17 Mo1 F5 K4 -126.0(2) . 2_564
O17 K4 F8 Mo2 -103.6(2) 2 2_565
O17 K4 F8 K1 51.3(2) 2 .
O17 K4 F8 K2 149.27(18) 2 2_565
O17 K4 F11 Mo2 173.0(3) 2 .
O17 K4 F11 K1 -70.43(17) 2 .
O17 K4 F11 K3 28.64(18) 2 .
O18 Mo3 F2 K1 33.8(3) . 3_655
O18 Mo3 F2 K2 131.2(2) . 4
O18 Mo3 F2 K5 -113.8(2) . .
O18 Mo3 F13 K2 129.3(2) . 2
O18 Mo3 F13 K3 -8.2(6) . 2
O18 Mo3 F13 K6 -143.2(2) . 2
O18 K6 F12 Mo2 38.3(4) 2_564 .
O18 K6 F12 K2 -101.0(2) 2_564 .
O18 K6 F12 K3 159.7(2) 2_564 .
O19 Mo4 F1 K2 125.8(2) . 2_565
O19 Mo4 F1 K4 13.6(3) . 2_564
O19 Mo4 F1 K5 -123.6(2) . 1_565
O19 Mo4 F3 K1 -22.8(3) . .
O19 Mo4 F3 K2 -128.5(2) . 2_565
O19 Mo4 F3 K6 134.6(2) . 2_565
